# Electronic Supplementary Material (ESI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2015

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 987931'
_audit_update_record             
;
2015-11-22 deposited with the CCDC.
2015-11-30 downloaded from the CCDC.
;
_audit_creation_date             2015-11-21
_audit_creation_method           
;
Olex2 1.2
(compiled 2015.09.30 svn.r3233 for OlexSys, GUI svn.r5103)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         
'0.5(C12 H24 As4 K8 N4 Ni4 O230 P12 W56), 19(O)'
_chemical_formula_sum            'C6 H74 As2 K4 N2 Ni2 O134 P6 W28'
_chemical_formula_weight         8075.57
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 1 2/c 1'
_space_group_name_Hall           '-C 2yc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   29.917(2)
_cell_length_b                   27.6712(18)
_cell_length_c                   20.6670(13)
_cell_angle_alpha                90
_cell_angle_beta                 122.3180(10)
_cell_angle_gamma                90
_cell_volume                     14458.8(16)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    8682
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.92
_cell_measurement_theta_min      2.17
_shelx_estimated_absorpt_T_max   0.103
_shelx_estimated_absorpt_T_min   0.040
_exptl_absorpt_coefficient_mu    23.170
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.3637
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2008/1 (Bruker,2008) was used for absorption correction.
wR2(int) was 0.1439 before and 0.0582 after correction.
The Ratio of minimum to maximum transmission is 0.4877.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'light green'
_exptl_crystal_density_diffrn    3.703
_exptl_crystal_density_meas      .
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             14168
_exptl_crystal_size_max          0.39
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.18
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0559
_diffrn_reflns_av_unetI/netI     0.0656
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -35
_diffrn_reflns_limit_k_max       33
_diffrn_reflns_limit_k_min       -31
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            37338
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_theta_full        25.100
_diffrn_reflns_theta_max         25.100
_diffrn_reflns_theta_min         1.878
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                9600
_reflns_number_total             12800
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         4.229
_refine_diff_density_min         -2.042
_refine_diff_density_rms         0.373
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.997
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     789
_refine_ls_number_reflns         12800
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0669
_refine_ls_R_factor_gt           0.0438
_refine_ls_restrained_S_all      0.997
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0648P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1094
_refine_ls_wR_factor_ref         0.1182
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H,H) groups
2. Restrained distances
 O5W-O10W
 2.7 with sigma of 0.02
3. Others
 Fixed Sof: O7W(0.6) O8W(0.4) O9W(0.5) O10W(0.5) O11W(0.5) O12W(0.5) O14W(0.5)
 O15W(0.5) O16W(0.5) O17W(0.5)
4.a Secondary CH2 refined with riding coordinates:
 C1(H1A,H1B), C2(H2A,H2B), C3(H3A,H3B)
;
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.18341(3) 0.56864(2) 0.84182(3) 0.02467(15) Uani 1 1 d . . . . .
W2 W 0.31651(3) 0.56567(2) 0.94572(3) 0.02447(15) Uani 1 1 d . . . . .
W3 W 0.24809(3) 0.48509(2) 0.80263(3) 0.02728(16) Uani 1 1 d . . . . .
W4 W 0.39064(2) 0.60760(2) 0.86063(3) 0.02616(15) Uani 1 1 d . . . . .
W5 W 0.32471(3) 0.52383(2) 0.71695(4) 0.02861(16) Uani 1 1 d . . . . .
W6 W 0.32664(3) 0.64121(2) 0.67517(3) 0.02538(15) Uani 1 1 d . . . . .
W7 W 0.17823(3) 0.64230(2) 0.55819(3) 0.02505(15) Uani 1 1 d . . . . .
W8 W 0.17868(3) 0.52542(2) 0.60223(3) 0.02890(16) Uani 1 1 d . . . . .
W9 W 0.11021(3) 0.60699(2) 0.63715(3) 0.02744(15) Uani 1 1 d . . . . .
W10 W 0.33241(3) 0.76323(2) 0.74441(3) 0.02465(15) Uani 1 1 d . . . . .
W11 W 0.18564(2) 0.76499(2) 0.62849(3) 0.02301(14) Uani 1 1 d . . . . .
W12 W 0.11917(2) 0.73093(2) 0.70936(3) 0.02292(14) Uani 1 1 d . . . . .
W13 W 0.18800(2) 0.69043(2) 0.91149(3) 0.02044(14) Uani 1 1 d . . . . .
W14 W 0.32243(2) 0.68930(2) 1.01442(3) 0.02132(14) Uani 1 1 d . . . . .
As1 As 0.25080(6) 0.62160(5) 0.76073(8) 0.0184(3) Uani 1 1 d . . . . .
Ni1 Ni 0.38461(6) 0.73346(5) 0.91775(9) 0.0129(3) Uani 1 1 d . . . . .
P1 P 0.25604(14) 0.74625(12) 0.83058(19) 0.0157(7) Uani 1 1 d . . . . .
P2 P 0.36229(16) 0.84827(13) 0.8747(2) 0.0264(9) Uani 1 1 d . . . . .
P3 P 0.14894(16) 0.84755(13) 0.7096(2) 0.0258(9) Uani 1 1 d . . . . .
K1 K 0.0440(2) 0.6824(2) 0.9161(3) 0.0814(17) Uani 1 1 d . . . . .
K2 K 0.0858(4) 0.7552(3) 0.3778(5) 0.154(3) Uani 1 1 d . . . . .
N1 N 0.2560(5) 0.8482(4) 0.8217(7) 0.028(3) Uani 1 1 d . . . . .
O1 O 0.1402(5) 0.5549(4) 0.8681(6) 0.039(3) Uani 1 1 d . . . . .
O2 O 0.2487(4) 0.5602(3) 0.9377(5) 0.026(2) Uani 1 1 d . . . . .
O3 O 0.1939(4) 0.5008(3) 0.8205(6) 0.031(2) Uani 1 1 d . . . . .
O4 O 0.1871(4) 0.6350(3) 0.8504(5) 0.021(2) Uani 1 1 d . . . . .
O5 O 0.1358(4) 0.5758(3) 0.7313(5) 0.029(2) Uani 1 1 d . . . . .
O6 O 0.2498(4) 0.5716(3) 0.8158(5) 0.022(2) Uani 1 1 d . . . . .
O7 O 0.3582(5) 0.5491(4) 1.0385(6) 0.042(3) Uani 1 1 d . . . . .
O8 O 0.3012(4) 0.4984(3) 0.9051(6) 0.033(3) Uani 1 1 d . . . . .
O9 O 0.3622(4) 0.5703(3) 0.9081(5) 0.025(2) Uani 1 1 d . . . . .
O10 O 0.3142(4) 0.6316(3) 0.9530(5) 0.021(2) Uani 1 1 d . . . . .
O11 O 0.2464(5) 0.4229(3) 0.8054(6) 0.036(3) Uani 1 1 d . . . . .
O12 O 0.1949(4) 0.4968(3) 0.6937(5) 0.030(2) Uani 1 1 d . . . . .
O13 O 0.2984(4) 0.4948(3) 0.7733(5) 0.027(2) Uani 1 1 d . . . . .
O14 O 0.4585(4) 0.5997(4) 0.9222(6) 0.038(3) Uani 1 1 d . . . . .
O15 O 0.3846(4) 0.5430(4) 0.8039(6) 0.033(3) Uani 1 1 d . . . . .
O16 O 0.3909(4) 0.6354(3) 0.7729(6) 0.032(3) Uani 1 1 d . . . . .
O17 O 0.3796(4) 0.6631(3) 0.8902(6) 0.029(2) Uani 1 1 d . . . . .
O18 O 0.3056(4) 0.6009(3) 0.7549(6) 0.031(2) Uani 1 1 d . . . . .
O19 O 0.3457(5) 0.4753(3) 0.6889(7) 0.042(3) Uani 1 1 d . . . . .
O20 O 0.3312(4) 0.5741(3) 0.6576(6) 0.031(2) Uani 1 1 d . . . . .
O21 O 0.2489(4) 0.5258(4) 0.6328(6) 0.038(3) Uani 1 1 d . . . . .
O22 O 0.3505(5) 0.6642(4) 0.6229(6) 0.039(3) Uani 1 1 d . . . . .
O23 O 0.2519(4) 0.6367(3) 0.6008(5) 0.028(2) Uani 1 1 d . . . . .
O24 O 0.3122(4) 0.6993(3) 0.7094(6) 0.032(3) Uani 1 1 d . . . . .
O25 O 0.1568(5) 0.6690(4) 0.4715(6) 0.044(3) Uani 1 1 d . . . . .
O26 O 0.1672(4) 0.5770(3) 0.5297(6) 0.031(2) Uani 1 1 d . . . . .
O27 O 0.1157(4) 0.6415(3) 0.5600(5) 0.027(2) Uani 1 1 d . . . . .
O28 O 0.1968(4) 0.7014(3) 0.6212(5) 0.026(2) Uani 1 1 d . . . . .
O29 O 0.1526(5) 0.4782(4) 0.5381(6) 0.043(3) Uani 1 1 d . . . . .
O30 O 0.1979(4) 0.6011(3) 0.6686(5) 0.021(2) Uani 1 1 d . . . . .
O31 O 0.1125(4) 0.5487(4) 0.5896(6) 0.037(3) Uani 1 1 d . . . . .
O32 O 0.0430(4) 0.6090(4) 0.5989(6) 0.041(3) Uani 1 1 d . . . . .
O33 O 0.1299(4) 0.6670(3) 0.6950(5) 0.027(2) Uani 1 1 d . . . . .
O34 O 0.3507(4) 0.7818(4) 0.6839(6) 0.035(3) Uani 1 1 d . . . . .
O35 O 0.2564(4) 0.7827(3) 0.6814(5) 0.025(2) Uani 1 1 d . . . . .
O36 O 0.3928(4) 0.7482(3) 0.8277(5) 0.027(2) Uani 1 1 d . . . . .
O37 O 0.3038(4) 0.7408(3) 0.8266(5) 0.022(2) Uani 1 1 d . . . . .
O38 O 0.3363(4) 0.8293(3) 0.7913(5) 0.026(2) Uani 1 1 d . . . . .
O39 O 0.1629(4) 0.7847(4) 0.5364(5) 0.034(3) Uani 1 1 d . . . . .
O40 O 0.1198(4) 0.7505(3) 0.6208(5) 0.024(2) Uani 1 1 d . . . . .
O41 O 0.2059(4) 0.7418(3) 0.7511(5) 0.020(2) Uani 1 1 d . . . . .
O42 O 0.1738(4) 0.8305(3) 0.6668(5) 0.030(2) Uani 1 1 d . . . . .
O43 O 0.0515(4) 0.7319(4) 0.6699(5) 0.033(3) Uani 1 1 d . . . . .
O44 O 0.1433(4) 0.7204(3) 0.8118(5) 0.024(2) Uani 1 1 d . . . . .
O45 O 0.1304(4) 0.8033(3) 0.7362(5) 0.028(2) Uani 1 1 d . . . . .
O46 O 0.1437(4) 0.6664(4) 0.9304(6) 0.034(3) Uani 1 1 d . . . . .
O47 O 0.2511(4) 0.6682(3) 0.9936(5) 0.021(2) Uani 1 1 d . . . . .
O48 O 0.2554(4) 0.7139(3) 0.8901(5) 0.022(2) Uani 1 1 d . . . . .
O49 O 0.3626(4) 0.6647(4) 1.1026(5) 0.034(3) Uani 1 1 d . . . . .
O50 O 0.3055(4) 0.7482(3) 1.0465(5) 0.025(2) Uani 1 1 d . . . . .
O51 O 0.3676(4) 0.7178(3) 0.9962(5) 0.028(2) Uani 1 1 d . . . . .
O52 O 0.4622(5) 0.7336(4) 0.9964(6) 0.047(3) Uani 1 1 d . . . . .
O53 O 0.3812(4) 0.8079(3) 0.9316(5) 0.028(2) Uani 1 1 d . . . . .
O54 O 0.4016(4) 0.8874(4) 0.8922(6) 0.041(3) Uani 1 1 d . . . . .
O55 O 0.1063(4) 0.8845(4) 0.6693(6) 0.040(3) Uani 1 1 d . . . . .
C1 C 0.2572(5) 0.8052(4) 0.8681(7) 0.017(3) Uani 1 1 d . . . . .
H1A H 0.2272 0.8077 0.8738 0.021 Uiso 1 1 calc R . . . .
H1B H 0.2889 0.8076 0.9189 0.021 Uiso 1 1 calc R . . . .
C2 C 0.3049(6) 0.8784(5) 0.8684(8) 0.026(3) Uani 1 1 d . . . . .
H2A H 0.3117 0.8829 0.9194 0.031 Uiso 1 1 calc R . . . .
H2B H 0.2997 0.9099 0.8449 0.031 Uiso 1 1 calc R . . . .
C3 C 0.2045(6) 0.8771(5) 0.7919(9) 0.028(3) Uani 1 1 d . . . . .
H3A H 0.2088 0.9094 0.7776 0.034 Uiso 1 1 calc R . . . .
H3B H 0.1974 0.8801 0.8323 0.034 Uiso 1 1 calc R . . . .
O1W O 0.7513(7) 0.9535(6) 0.9885(9) 0.090(5) Uiso 1 1 d . . . . .
O2W O 0.8316(6) 0.8924(5) 0.9668(7) 0.063(4) Uiso 1 1 d . . . . .
O3W O 0.0784(5) 0.9107(5) 0.7951(7) 0.057(3) Uiso 1 1 d . . . . .
O4W O 0.0397(7) 0.5367(6) 0.0059(9) 0.089(5) Uiso 1 1 d . . . . .
O5W O 0.6268(7) 0.9574(6) 0.8812(10) 0.098(6) Uiso 1 1 d D . . . .
O6W O 0.0347(8) 0.7271(7) 0.4652(10) 0.106(6) Uiso 1 1 d . . . . .
O7W O 0.2496(10) 0.6641(9) 0.4546(13) 0.062(6) Uiso 0.6 1 d . . P A 1
O8W O 0.231(2) 0.6405(17) 0.414(3) 0.101(15) Uiso 0.4 1 d . . P B 2
O9W O 0.9932(11) 0.8500(9) 0.9336(14) 0.056(7) Uiso 0.5 1 d . . P . .
O10W O 0.6629(9) 0.8884(7) 0.8326(12) 0.042(6) Uiso 0.5 1 d D . P . .
O11W O 0.0474(11) 0.7554(9) 0.8243(15) 0.062(7) Uiso 0.5 1 d . . P . .
O12W O 0.0916(11) 0.5399(9) 0.1934(14) 0.057(7) Uiso 0.5 1 d . . P . .
O13W O 0.0936(8) 0.0403(7) 0.0698(10) 0.107(6) Uiso 1 1 d . . . . .
O14W O 0.8915(10) 0.9517(8) 1.0887(14) 0.052(6) Uiso 0.5 1 d . . P . .
O15W O 0.4656(14) 0.7190(12) 0.7847(19) 0.096(11) Uiso 0.5 1 d . . P . .
O16W O 0.4927(14) 0.8620(11) 0.8988(19) 0.089(10) Uiso 0.5 1 d . . P . .
O17W O 0.0678(9) 0.5829(8) -0.0826(12) 0.044(6) Uiso 0.5 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.690(10) . ?
W1 O2 1.914(10) . ?
W1 O3 1.992(9) . ?
W1 O4 1.842(8) . ?
W1 O5 1.950(9) . ?
W1 O6 2.320(10) . ?
W2 O2 1.950(11) . ?
W2 O6 2.343(9) . ?
W2 O7 1.699(10) . ?
W2 O8 1.992(9) . ?
W2 O9 1.903(10) . ?
W2 O10 1.835(8) . ?
W3 O3 1.895(11) . ?
W3 O6 2.408(8) . ?
W3 O8 1.884(10) . ?
W3 O11 1.725(10) . ?
W3 O12 1.969(10) . ?
W3 O13 1.919(10) . ?
W4 O9 1.910(9) . ?
W4 O14 1.739(10) . ?
W4 O15 2.093(10) . ?
W4 O16 1.974(10) . ?
W4 O17 1.750(9) . ?
W4 O18 2.311(11) . ?
W5 O13 1.897(9) . ?
W5 O15 1.810(10) . ?
W5 O18 2.444(9) . ?
W5 O19 1.710(10) . ?
W5 O20 1.933(9) . ?
W5 O21 1.988(11) . ?
W6 O16 1.911(11) . ?
W6 O18 2.337(10) . ?
W6 O20 1.912(10) . ?
W6 O22 1.704(10) . ?
W6 O23 1.923(10) . ?
W6 O24 1.897(9) . ?
W7 O23 1.894(10) . ?
W7 O25 1.714(10) . ?
W7 O26 1.873(9) . ?
W7 O27 1.893(10) . ?
W7 O28 1.977(9) . ?
W7 O30 2.327(8) . ?
W8 O12 1.858(9) . ?
W8 O21 1.842(11) . ?
W8 O26 1.964(10) . ?
W8 O29 1.722(10) . ?
W8 O30 2.398(9) . ?
W8 O31 1.963(12) . ?
W9 O5 1.878(9) . ?
W9 O27 1.938(9) . ?
W9 O30 2.348(10) . ?
W9 O31 1.908(10) . ?
W9 O32 1.725(11) . ?
W9 O33 1.944(9) . ?
W10 O24 1.884(10) . ?
W10 O34 1.692(10) . ?
W10 O35 1.998(9) . ?
W10 O36 1.754(9) . ?
W10 O37 2.356(9) . ?
W10 O38 2.043(9) . ?
W11 O28 1.812(9) . ?
W11 O35 1.855(9) . ?
W11 O39 1.731(9) . ?
W11 O40 1.931(10) . ?
W11 O41 2.358(8) . ?
W11 O42 2.084(10) . ?
W12 O33 1.850(9) . ?
W12 O40 1.919(9) . ?
W12 O41 2.274(10) . ?
W12 O43 1.733(10) . ?
W12 O44 1.859(9) . ?
W12 O45 2.058(9) . ?
W13 O4 1.978(8) . ?
W13 O44 1.943(9) . ?
W13 O46 1.704(11) . ?
W13 O47 1.842(9) . ?
W13 O48 2.375(10) . ?
W13 O50 1.870(8) 7_567 ?
W14 O10 1.972(8) . ?
W14 O47 2.025(10) . ?
W14 O48 2.361(9) . ?
W14 O49 1.699(9) . ?
W14 O50 1.927(8) . ?
W14 O51 1.772(10) . ?
As1 O6 1.802(8) . ?
As1 O18 1.800(10) . ?
As1 O30 1.797(9) . ?
Ni1 K1 3.732(5) 7_567 ?
Ni1 O17 2.010(9) . ?
Ni1 O36 2.043(9) . ?
Ni1 O37 2.136(10) . ?
Ni1 O51 1.988(10) . ?
Ni1 O52 1.998(11) . ?
Ni1 O53 2.090(9) . ?
P1 O37 1.483(10) . ?
P1 O41 1.526(9) . ?
P1 O48 1.529(9) . ?
P1 C1 1.799(12) . ?
P2 K1 3.782(6) 7_567 ?
P2 O38 1.556(10) . ?
P2 O53 1.497(10) . ?
P2 O54 1.494(11) . ?
P2 C2 1.849(16) . ?
P3 O42 1.503(11) . ?
P3 O45 1.559(10) . ?
P3 O55 1.493(10) . ?
P3 C3 1.817(16) . ?
K1 Ni1 3.732(5) 7_567 ?
K1 P2 3.782(6) 7_567 ?
K1 O32 3.182(13) 2_556 ?
K1 O43 2.786(11) 2_556 ?
K1 O46 2.872(12) . ?
K1 O52 3.010(12) 7_567 ?
K1 O53 2.729(10) 7_567 ?
K1 O11W 2.81(3) . ?
K1 O17W 2.84(2) 1_556 ?
K2 K2 5.026(19) 2 ?
K2 O22 2.938(14) 7_566 ?
K2 O25 3.092(15) . ?
K2 O34 2.978(14) 7_566 ?
K2 O39 2.940(14) . ?
K2 O6W 3.03(2) . ?
K2 O15W 3.12(4) 8_465 ?
K2 O15W 2.94(3) 7_566 ?
N1 C1 1.517(16) . ?
N1 C2 1.503(18) . ?
N1 C3 1.543(18) . ?
O22 K2 2.938(14) 7_566 ?
O32 K1 3.182(13) 2_556 ?
O34 K2 2.978(14) 7_566 ?
O43 K1 2.786(11) 2_556 ?
O50 W13 1.870(8) 7_567 ?
O52 K1 3.010(12) 7_567 ?
O53 K1 2.730(10) 7_567 ?
C1 H1A 0.9700 . ?
C1 H1B 0.9700 . ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
O15W K2 3.12(4) 8_566 ?
O15W K2 2.94(3) 7_566 ?
O17W K1 2.84(2) 1_554 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O2 99.9(5) . . ?
O1 W1 O3 95.5(5) . . ?
O1 W1 O4 102.2(5) . . ?
O1 W1 O5 101.2(5) . . ?
O1 W1 O6 168.0(4) . . ?
O2 W1 O3 85.4(4) . . ?
O2 W1 O5 158.0(4) . . ?
O2 W1 O6 73.6(4) . . ?
O3 W1 O6 74.1(4) . . ?
O4 W1 O2 92.7(4) . . ?
O4 W1 O3 162.3(4) . . ?
O4 W1 O5 88.9(4) . . ?
O4 W1 O6 88.4(4) . . ?
O5 W1 O3 86.5(4) . . ?
O5 W1 O6 84.6(4) . . ?
O2 W2 O6 72.4(4) . . ?
O2 W2 O8 84.1(4) . . ?
O7 W2 O2 100.2(5) . . ?
O7 W2 O6 166.9(4) . . ?
O7 W2 O8 95.0(5) . . ?
O7 W2 O9 103.0(5) . . ?
O7 W2 O10 102.3(4) . . ?
O8 W2 O6 73.8(3) . . ?
O9 W2 O2 155.7(4) . . ?
O9 W2 O6 83.4(4) . . ?
O9 W2 O8 86.8(4) . . ?
O10 W2 O2 90.1(4) . . ?
O10 W2 O6 88.7(3) . . ?
O10 W2 O8 162.4(4) . . ?
O10 W2 O9 91.9(4) . . ?
O3 W3 O6 73.6(4) . . ?
O3 W3 O12 86.1(4) . . ?
O3 W3 O13 157.9(4) . . ?
O8 W3 O3 91.8(5) . . ?
O8 W3 O6 74.0(3) . . ?
O8 W3 O12 159.0(4) . . ?
O8 W3 O13 89.7(4) . . ?
O11 W3 O3 100.4(5) . . ?
O11 W3 O6 171.4(4) . . ?
O11 W3 O8 100.4(4) . . ?
O11 W3 O12 100.5(4) . . ?
O11 W3 O13 101.0(5) . . ?
O12 W3 O6 85.4(3) . . ?
O13 W3 O6 85.7(3) . . ?
O13 W3 O12 84.6(4) . . ?
O9 W4 O15 84.1(4) . . ?
O9 W4 O16 154.8(4) . . ?
O9 W4 O18 82.8(4) . . ?
O14 W4 O9 102.8(5) . . ?
O14 W4 O15 91.1(4) . . ?
O14 W4 O16 98.3(5) . . ?
O14 W4 O17 102.7(5) . . ?
O14 W4 O18 161.1(4) . . ?
O15 W4 O18 71.3(4) . . ?
O16 W4 O15 82.0(4) . . ?
O16 W4 O18 72.9(4) . . ?
O17 W4 O9 94.3(4) . . ?
O17 W4 O15 166.1(4) . . ?
O17 W4 O16 94.2(4) . . ?
O17 W4 O18 94.7(4) . . ?
O13 W5 O18 85.9(4) . . ?
O13 W5 O20 155.6(4) . . ?
O13 W5 O21 84.0(5) . . ?
O15 W5 O13 91.7(5) . . ?
O15 W5 O18 72.7(4) . . ?
O15 W5 O20 92.1(5) . . ?
O15 W5 O21 157.1(4) . . ?
O19 W5 O13 102.8(5) . . ?
O19 W5 O15 102.6(5) . . ?
O19 W5 O18 170.4(5) . . ?
O19 W5 O20 99.8(5) . . ?
O19 W5 O21 100.3(5) . . ?
O20 W5 O18 72.3(4) . . ?
O20 W5 O21 83.1(4) . . ?
O21 W5 O18 84.5(4) . . ?
O16 W6 O18 73.3(4) . . ?
O16 W6 O20 89.2(4) . . ?
O16 W6 O23 157.2(4) . . ?
O20 W6 O18 75.2(4) . . ?
O20 W6 O23 87.5(4) . . ?
O22 W6 O16 100.1(5) . . ?
O22 W6 O18 170.6(5) . . ?
O22 W6 O20 98.3(5) . . ?
O22 W6 O23 102.7(5) . . ?
O22 W6 O24 100.1(5) . . ?
O23 W6 O18 84.0(4) . . ?
O24 W6 O16 88.7(4) . . ?
O24 W6 O18 86.6(4) . . ?
O24 W6 O20 161.5(4) . . ?
O24 W6 O23 87.4(4) . . ?
O23 W7 O28 85.1(4) . . ?
O23 W7 O30 83.2(4) . . ?
O25 W7 O23 102.3(5) . . ?
O25 W7 O26 100.5(5) . . ?
O25 W7 O27 101.8(5) . . ?
O25 W7 O28 98.5(4) . . ?
O25 W7 O30 173.3(5) . . ?
O26 W7 O23 91.8(4) . . ?
O26 W7 O27 89.1(4) . . ?
O26 W7 O28 161.0(4) . . ?
O26 W7 O30 75.3(4) . . ?
O27 W7 O23 155.2(4) . . ?
O27 W7 O28 86.0(4) . . ?
O27 W7 O30 73.1(4) . . ?
O28 W7 O30 85.7(3) . . ?
O12 W8 O26 158.5(4) . . ?
O12 W8 O30 86.4(3) . . ?
O12 W8 O31 88.4(5) . . ?
O21 W8 O12 91.3(5) . . ?
O21 W8 O26 87.7(5) . . ?
O21 W8 O30 85.3(4) . . ?
O21 W8 O31 158.2(4) . . ?
O26 W8 O30 72.1(3) . . ?
O29 W8 O12 103.0(4) . . ?
O29 W8 O21 103.4(5) . . ?
O29 W8 O26 98.1(5) . . ?
O29 W8 O30 166.8(4) . . ?
O29 W8 O31 97.9(5) . . ?
O31 W8 O26 84.7(4) . . ?
O31 W8 O30 72.9(4) . . ?
O5 W9 O27 155.8(4) . . ?
O5 W9 O30 84.6(4) . . ?
O5 W9 O31 92.2(4) . . ?
O5 W9 O33 86.2(4) . . ?
O27 W9 O30 71.9(4) . . ?
O27 W9 O33 87.4(4) . . ?
O31 W9 O27 87.2(4) . . ?
O31 W9 O30 75.0(4) . . ?
O31 W9 O33 162.9(5) . . ?
O32 W9 O5 102.6(5) . . ?
O32 W9 O27 101.4(5) . . ?
O32 W9 O30 170.5(4) . . ?
O32 W9 O31 98.3(5) . . ?
O32 W9 O33 98.6(5) . . ?
O33 W9 O30 87.9(4) . . ?
O24 W10 O35 89.1(4) . . ?
O24 W10 O37 82.2(4) . . ?
O24 W10 O38 161.3(4) . . ?
O34 W10 O24 99.6(5) . . ?
O34 W10 O35 98.2(4) . . ?
O34 W10 O36 103.2(5) . . ?
O34 W10 O37 177.0(4) . . ?
O34 W10 O38 96.8(5) . . ?
O35 W10 O37 79.3(4) . . ?
O35 W10 O38 79.9(4) . . ?
O36 W10 O24 96.0(4) . . ?
O36 W10 O35 156.9(4) . . ?
O36 W10 O37 79.0(4) . . ?
O36 W10 O38 88.8(4) . . ?
O38 W10 O37 81.1(3) . . ?
O28 W11 O35 95.9(4) . . ?
O28 W11 O40 90.9(4) . . ?
O28 W11 O41 82.7(4) . . ?
O28 W11 O42 162.3(4) . . ?
O35 W11 O40 153.5(4) . . ?
O35 W11 O41 83.2(4) . . ?
O35 W11 O42 85.3(4) . . ?
O39 W11 O28 101.3(5) . . ?
O39 W11 O35 102.7(5) . . ?
O39 W11 O40 101.0(4) . . ?
O39 W11 O41 172.4(4) . . ?
O39 W11 O42 95.6(4) . . ?
O40 W11 O41 72.3(4) . . ?
O40 W11 O42 80.7(4) . . ?
O42 W11 O41 80.0(3) . . ?
O33 W12 O40 91.5(4) . . ?
O33 W12 O41 85.8(4) . . ?
O33 W12 O44 92.2(4) . . ?
O33 W12 O45 163.1(4) . . ?
O40 W12 O41 74.5(4) . . ?
O40 W12 O45 84.2(4) . . ?
O43 W12 O33 101.4(5) . . ?
O43 W12 O40 98.8(4) . . ?
O43 W12 O41 170.4(4) . . ?
O43 W12 O44 100.5(5) . . ?
O43 W12 O45 95.4(5) . . ?
O44 W12 O40 159.2(4) . . ?
O44 W12 O41 85.4(4) . . ?
O44 W12 O45 86.4(4) . . ?
O45 W12 O41 77.3(4) . . ?
O4 W13 O48 79.4(3) . . ?
O44 W13 O4 83.6(4) . . ?
O44 W13 O48 81.8(4) . . ?
O46 W13 O4 95.5(4) . . ?
O46 W13 O44 103.3(4) . . ?
O46 W13 O47 101.4(4) . . ?
O46 W13 O48 172.4(4) . . ?
O46 W13 O50 98.6(5) . 7_567 ?
O47 W13 O4 89.3(4) . . ?
O47 W13 O44 154.8(4) . . ?
O47 W13 O48 73.1(4) . . ?
O47 W13 O50 94.2(4) . 7_567 ?
O50 W13 O4 164.5(4) 7_567 . ?
O50 W13 O44 86.9(4) 7_567 . ?
O50 W13 O48 87.1(4) 7_567 . ?
O10 W14 O47 82.8(4) . . ?
O10 W14 O48 78.0(3) . . ?
O47 W14 O48 70.5(3) . . ?
O49 W14 O10 98.1(4) . . ?
O49 W14 O47 100.0(5) . . ?
O49 W14 O48 170.0(4) . . ?
O49 W14 O50 97.7(4) . . ?
O49 W14 O51 103.0(5) . . ?
O50 W14 O10 160.3(4) . . ?
O50 W14 O47 82.8(4) . . ?
O50 W14 O48 84.5(4) . . ?
O51 W14 O10 94.0(4) . . ?
O51 W14 O47 157.1(4) . . ?
O51 W14 O48 86.6(4) . . ?
O51 W14 O50 93.9(4) . . ?
O18 As1 O6 97.0(4) . . ?
O30 As1 O6 97.2(4) . . ?
O30 As1 O18 98.4(5) . . ?
O17 Ni1 K1 141.6(3) . 7_567 ?
O17 Ni1 O36 87.9(4) . . ?
O17 Ni1 O37 88.0(4) . . ?
O17 Ni1 O53 172.4(4) . . ?
O36 Ni1 K1 115.1(3) . 7_567 ?
O36 Ni1 O37 78.9(4) . . ?
O36 Ni1 O53 88.1(4) . . ?
O37 Ni1 K1 125.0(2) . 7_567 ?
O51 Ni1 K1 69.9(3) . 7_567 ?
O51 Ni1 O17 90.4(4) . . ?
O51 Ni1 O36 173.2(4) . . ?
O51 Ni1 O37 94.5(4) . . ?
O51 Ni1 O52 91.7(5) . . ?
O51 Ni1 O53 92.9(4) . . ?
O52 Ni1 K1 53.5(3) . 7_567 ?
O52 Ni1 O17 96.4(4) . . ?
O52 Ni1 O36 95.1(5) . . ?
O52 Ni1 O37 172.5(4) . . ?
O52 Ni1 O53 90.4(4) . . ?
O53 Ni1 K1 45.9(3) . 7_567 ?
O53 Ni1 O37 84.9(4) . . ?
O37 P1 O41 110.8(5) . . ?
O37 P1 O48 114.3(5) . . ?
O37 P1 C1 108.6(6) . . ?
O41 P1 O48 113.0(5) . . ?
O41 P1 C1 108.6(6) . . ?
O48 P1 C1 100.9(6) . . ?
O38 P2 K1 144.8(4) . 7_567 ?
O38 P2 C2 100.3(6) . . ?
O53 P2 K1 36.5(4) . 7_567 ?
O53 P2 O38 112.0(5) . . ?
O53 P2 C2 109.8(6) . . ?
O54 P2 K1 83.0(5) . 7_567 ?
O54 P2 O38 112.0(6) . . ?
O54 P2 O53 115.6(6) . . ?
O54 P2 C2 105.8(6) . . ?
C2 P2 K1 105.9(5) . 7_567 ?
O42 P3 O45 110.0(5) . . ?
O42 P3 C3 101.5(6) . . ?
O45 P3 C3 110.1(6) . . ?
O55 P3 O42 115.4(6) . . ?
O55 P3 O45 112.1(6) . . ?
O55 P3 C3 107.2(6) . . ?
Ni1 K1 P2 51.58(9) 7_567 7_567 ?
O32 K1 Ni1 121.6(3) 2_556 7_567 ?
O32 K1 P2 92.1(2) 2_556 7_567 ?
O43 K1 Ni1 99.7(3) 2_556 7_567 ?
O43 K1 P2 136.1(3) 2_556 7_567 ?
O43 K1 O32 75.3(3) 2_556 2_556 ?
O43 K1 O46 142.7(4) 2_556 . ?
O43 K1 O52 68.5(3) 2_556 7_567 ?
O43 K1 O11W 67.1(6) 2_556 . ?
O43 K1 O17W 130.4(6) 2_556 1_556 ?
O46 K1 Ni1 87.1(2) . 7_567 ?
O46 K1 P2 75.7(2) . 7_567 ?
O46 K1 O32 131.4(3) . 2_556 ?
O46 K1 O52 116.8(4) . 7_567 ?
O52 K1 Ni1 32.3(2) 7_567 7_567 ?
O52 K1 P2 74.5(2) 7_567 7_567 ?
O52 K1 O32 104.0(4) 7_567 2_556 ?
O53 K1 Ni1 33.4(2) 7_567 7_567 ?
O53 K1 P2 19.1(2) 7_567 7_567 ?
O53 K1 O32 107.4(3) 7_567 2_556 ?
O53 K1 O43 128.1(4) 7_567 2_556 ?
O53 K1 O46 74.3(3) 7_567 . ?
O53 K1 O52 60.5(3) 7_567 7_567 ?
O53 K1 O11W 113.8(6) 7_567 . ?
O53 K1 O17W 92.2(5) 7_567 1_556 ?
O11W K1 Ni1 87.9(6) . 7_567 ?
O11W K1 P2 131.3(6) . 7_567 ?
O11W K1 O32 135.7(6) . 2_556 ?
O11W K1 O46 76.6(6) . . ?
O11W K1 O52 83.5(6) . 7_567 ?
O11W K1 O17W 127.1(7) . 1_556 ?
O17W K1 Ni1 125.4(5) 1_556 7_567 ?
O17W K1 P2 75.1(5) 1_556 7_567 ?
O17W K1 O32 64.5(5) 1_556 2_556 ?
O17W K1 O46 66.9(5) 1_556 . ?
O17W K1 O52 147.0(5) 1_556 7_567 ?
O22 K2 K2 107.2(3) 7_566 2 ?
O22 K2 O25 111.0(4) 7_566 . ?
O22 K2 O34 72.3(3) 7_566 7_566 ?
O22 K2 O39 70.8(4) 7_566 . ?
O22 K2 O6W 137.3(5) 7_566 . ?
O22 K2 O15W 111.1(7) 7_566 8_465 ?
O25 K2 K2 129.2(3) . 2 ?
O25 K2 O15W 137.9(7) . 8_465 ?
O34 K2 K2 94.4(3) 7_566 2 ?
O34 K2 O25 67.7(4) 7_566 . ?
O34 K2 O6W 143.9(5) 7_566 . ?
O34 K2 O15W 127.1(7) 7_566 8_465 ?
O39 K2 K2 157.4(4) . 2 ?
O39 K2 O25 69.4(3) . . ?
O39 K2 O34 105.8(4) . 7_566 ?
O39 K2 O6W 75.6(4) . . ?
O39 K2 O15W 125.6(7) . 8_465 ?
O6W K2 K2 94.0(5) . 2 ?
O6W K2 O25 79.9(5) . . ?
O6W K2 O15W 69.1(8) . 8_465 ?
O15W K2 K2 35.1(7) 7_566 2 ?
O15W K2 K2 32.8(6) 8_465 2 ?
O15W K2 O22 75.8(7) 7_566 7_566 ?
O15W K2 O25 131.9(8) 7_566 . ?
O15W K2 O34 70.0(8) 7_566 7_566 ?
O15W K2 O39 145.7(8) 7_566 . ?
O15W K2 O6W 128.5(9) 7_566 . ?
O15W K2 O15W 60.9(13) 7_566 8_465 ?
C1 N1 C3 109.9(11) . . ?
C2 N1 C1 110.1(10) . . ?
C2 N1 C3 113.0(11) . . ?
W1 O2 W2 121.2(5) . . ?
W3 O3 W1 120.8(5) . . ?
W1 O4 W13 144.5(5) . . ?
W9 O5 W1 153.9(6) . . ?
W1 O6 W2 92.4(3) . . ?
W1 O6 W3 91.2(3) . . ?
W2 O6 W3 90.8(3) . . ?
As1 O6 W1 118.7(4) . . ?
As1 O6 W2 119.1(4) . . ?
As1 O6 W3 134.3(4) . . ?
W3 O8 W2 121.5(5) . . ?
W2 O9 W4 149.4(5) . . ?
W2 O10 W14 149.4(5) . . ?
W8 O12 W3 147.7(6) . . ?
W5 O13 W3 154.9(6) . . ?
W5 O15 W4 123.3(5) . . ?
W6 O16 W4 120.5(5) . . ?
W4 O17 Ni1 161.7(6) . . ?
W4 O18 W5 92.6(3) . . ?
W4 O18 W6 93.0(4) . . ?
W6 O18 W5 89.6(3) . . ?
As1 O18 W4 119.5(5) . . ?
As1 O18 W5 132.6(5) . . ?
As1 O18 W6 119.6(5) . . ?
W6 O20 W5 122.4(5) . . ?
W8 O21 W5 149.1(6) . . ?
W6 O22 K2 141.2(6) . 7_566 ?
W7 O23 W6 158.9(6) . . ?
W10 O24 W6 148.0(6) . . ?
W7 O25 K2 137.3(6) . . ?
W7 O26 W8 122.1(5) . . ?
W7 O27 W9 122.8(5) . . ?
W11 O28 W7 149.2(6) . . ?
W7 O30 W8 90.6(3) . . ?
W7 O30 W9 92.0(3) . . ?
W9 O30 W8 90.6(3) . . ?
As1 O30 W7 120.2(4) . . ?
As1 O30 W8 133.5(5) . . ?
As1 O30 W9 119.4(4) . . ?
W9 O31 W8 121.4(5) . . ?
W9 O32 K1 139.2(5) . 2_556 ?
W12 O33 W9 153.3(5) . . ?
W10 O34 K2 138.1(5) . 7_566 ?
W11 O35 W10 148.8(5) . . ?
W10 O36 Ni1 112.3(5) . . ?
Ni1 O37 W10 89.2(3) . . ?
P1 O37 W10 138.2(5) . . ?
P1 O37 Ni1 129.1(5) . . ?
P2 O38 W10 134.0(6) . . ?
W11 O39 K2 138.7(5) . . ?
W12 O40 W11 120.7(5) . . ?
W12 O41 W11 92.5(3) . . ?
P1 O41 W11 132.4(6) . . ?
P1 O41 W12 133.2(5) . . ?
P3 O42 W11 137.3(6) . . ?
W12 O43 K1 146.5(6) . 2_556 ?
W12 O44 W13 154.5(6) . . ?
P3 O45 W12 135.0(6) . . ?
W13 O46 K1 144.0(5) . . ?
W13 O47 W14 122.9(4) . . ?
W14 O48 W13 91.7(3) . . ?
P1 O48 W13 133.3(5) . . ?
P1 O48 W14 132.5(6) . . ?
W13 O50 W14 161.2(6) 7_567 . ?
W14 O51 Ni1 145.8(5) . . ?
Ni1 O52 K1 94.2(4) . 7_567 ?
Ni1 O53 K1 100.7(4) . 7_567 ?
P2 O53 Ni1 130.8(5) . . ?
P2 O53 K1 124.4(5) . 7_567 ?
P1 C1 H1A 108.1 . . ?
P1 C1 H1B 108.1 . . ?
N1 C1 P1 116.7(9) . . ?
N1 C1 H1A 108.1 . . ?
N1 C1 H1B 108.1 . . ?
H1A C1 H1B 107.3 . . ?
P2 C2 H2A 109.6 . . ?
P2 C2 H2B 109.6 . . ?
N1 C2 P2 110.1(9) . . ?
N1 C2 H2A 109.6 . . ?
N1 C2 H2B 109.6 . . ?
H2A C2 H2B 108.2 . . ?
P3 C3 H3A 109.4 . . ?
P3 C3 H3B 109.4 . . ?
N1 C3 P3 111.1(9) . . ?
N1 C3 H3A 109.4 . . ?
N1 C3 H3B 109.4 . . ?
H3A C3 H3B 108.0 . . ?
K2 O15W K2 112.1(12) 7_566 8_566 ?

_shelx_SHELXL_version_number     2014/7
_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_2
_database_code_depnum_ccdc_archive 'CCDC 987933'
_audit_update_record             
;
2015-11-22 deposited with the CCDC.
2015-11-30 downloaded from the CCDC.
;
_audit_creation_date             2015-11-21
_audit_creation_method           
;
Olex2 1.2
(compiled 2015.09.30 svn.r3233 for OlexSys, GUI svn.r5103)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         
'0.5(C12 H24 As4 Co4 K8 N4 O230 P12 W56), 19(O)'
_chemical_formula_sum            'C6 H74 As2 Co2 K4 N2 O134 P6 W28'
_chemical_formula_weight         8076.05
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 1 2/c 1'
_space_group_name_Hall           '-C 2yc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   29.8801(12)
_cell_length_b                   27.6391(11)
_cell_length_c                   20.6261(8)
_cell_angle_alpha                90
_cell_angle_beta                 122.1840(10)
_cell_angle_gamma                90
_cell_volume                     14416.8(10)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    9163
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.12
_cell_measurement_theta_min      2.18
_shelx_estimated_absorpt_T_max   0.119
_shelx_estimated_absorpt_T_min   0.080
_exptl_absorpt_coefficient_mu    23.207
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.3681
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2008/1 (Bruker,2008) was used for absorption correction.
wR2(int) was 0.1437 before and 0.0489 after correction.
The Ratio of minimum to maximum transmission is 0.4936.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    3.714
_exptl_crystal_density_meas      .
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             14160
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.16
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0470
_diffrn_reflns_av_unetI/netI     0.0534
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_limit_h_max       35
_diffrn_reflns_limit_h_min       -35
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            37039
_diffrn_reflns_point_group_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.879
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                9726
_reflns_number_total             12743
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         4.108
_refine_diff_density_min         -1.625
_refine_diff_density_rms         0.314
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.022
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     791
_refine_ls_number_reflns         12743
_refine_ls_number_restraints     7
_refine_ls_R_factor_all          0.0594
_refine_ls_R_factor_gt           0.0381
_refine_ls_restrained_S_all      1.022
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0568P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0969
_refine_ls_wR_factor_ref         0.1038
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H,H) groups
2. Restrained distances
 O5W-O10W
 2.7 with sigma of 0.02
3. Rigid bond restraints
 N1, C3
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 P2, C2
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 Co1, O36
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 Co1, O37
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 Co1, O51
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 Co1, O52
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
4. Others
 Fixed Sof: O7W(0.6) O8W(0.4) O9W(0.5) O10W(0.5) O11W(0.5) O12W(0.5) O13W(0.5)
 O14W(0.5) O15W(0.5) O16W(0.5) O17W(0.5)
5.a Secondary CH2 refined with riding coordinates:
 C1(H1A,H1B), C2(H2A,H2B), C3(H3A,H3B)
;
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.18301(2) 0.56900(2) 0.84146(3) 0.02367(13) Uani 1 1 d . . . . .
W2 W 0.31578(2) 0.56568(2) 0.94488(3) 0.02352(13) Uani 1 1 d . . . . .
W3 W 0.24732(2) 0.48533(2) 0.80192(3) 0.02654(14) Uani 1 1 d . . . . .
W4 W 0.38990(2) 0.60732(2) 0.85948(3) 0.02545(13) Uani 1 1 d . . . . .
W5 W 0.32375(2) 0.52397(2) 0.71590(3) 0.02824(14) Uani 1 1 d . . . . .
W6 W 0.32606(2) 0.64137(2) 0.67459(3) 0.02507(13) Uani 1 1 d . . . . .
W7 W 0.17807(2) 0.64259(2) 0.55815(3) 0.02454(13) Uani 1 1 d . . . . .
W8 W 0.17808(2) 0.52575(2) 0.60183(3) 0.02833(14) Uani 1 1 d . . . . .
W9 W 0.11001(2) 0.60746(2) 0.63717(3) 0.02642(14) Uani 1 1 d . . . . .
W10 W 0.33193(2) 0.76337(2) 0.74344(3) 0.02493(13) Uani 1 1 d . . . . .
W11 W 0.18548(2) 0.76522(2) 0.62818(3) 0.02258(13) Uani 1 1 d . . . . .
W12 W 0.11917(2) 0.73129(2) 0.70951(3) 0.02224(13) Uani 1 1 d . . . . .
W13 W 0.18780(2) 0.69075(2) 0.91126(3) 0.01946(12) Uani 1 1 d . . . . .
W14 W 0.32206(2) 0.68902(2) 1.01429(3) 0.02052(12) Uani 1 1 d . . . . .
As1 As 0.25044(5) 0.62173(4) 0.76028(7) 0.0179(3) Uani 1 1 d . . . . .
Co1 Co 0.38566(6) 0.73345(5) 0.91876(8) 0.0114(3) Uani 1 1 d . U . . .
P1 P 0.25607(12) 0.74639(11) 0.83064(17) 0.0159(7) Uani 1 1 d . . . . .
P2 P 0.36196(14) 0.84876(12) 0.8736(2) 0.0257(8) Uani 1 1 d . U . . .
P3 P 0.14891(14) 0.84758(12) 0.7094(2) 0.0250(8) Uani 1 1 d . . . . .
K1 K 0.04315(17) 0.68118(19) 0.9155(2) 0.0764(14) Uani 1 1 d . . . . .
K2 K 0.0857(3) 0.7560(3) 0.3788(4) 0.149(3) Uani 1 1 d . . . . .
N1 N 0.2563(4) 0.8484(3) 0.8216(5) 0.019(2) Uani 1 1 d . U . . .
O1 O 0.1388(4) 0.5548(3) 0.8681(6) 0.040(3) Uani 1 1 d . . . . .
O2 O 0.2481(4) 0.5600(3) 0.9373(5) 0.027(2) Uani 1 1 d . . . . .
O3 O 0.1930(4) 0.5021(3) 0.8199(5) 0.033(2) Uani 1 1 d . . . . .
O4 O 0.1872(3) 0.6345(3) 0.8505(5) 0.022(2) Uani 1 1 d . . . . .
O5 O 0.1363(4) 0.5764(3) 0.7328(5) 0.027(2) Uani 1 1 d . . . . .
O6 O 0.2497(3) 0.5725(3) 0.8156(5) 0.022(2) Uani 1 1 d . . . . .
O7 O 0.3574(4) 0.5488(3) 1.0383(5) 0.035(2) Uani 1 1 d . . . . .
O8 O 0.2997(4) 0.4982(3) 0.9036(5) 0.030(2) Uani 1 1 d . . . . .
O9 O 0.3621(4) 0.5703(3) 0.9086(5) 0.029(2) Uani 1 1 d . . . . .
O10 O 0.3152(3) 0.6315(3) 0.9536(5) 0.023(2) Uani 1 1 d . . . . .
O11 O 0.2456(4) 0.4228(3) 0.8046(5) 0.036(2) Uani 1 1 d . . . . .
O12 O 0.1946(4) 0.4970(3) 0.6940(5) 0.028(2) Uani 1 1 d . . . . .
O13 O 0.2975(4) 0.4952(3) 0.7725(5) 0.027(2) Uani 1 1 d . . . . .
O14 O 0.4569(4) 0.6002(4) 0.9220(5) 0.041(3) Uani 1 1 d . . . . .
O15 O 0.3839(4) 0.5429(3) 0.8026(5) 0.030(2) Uani 1 1 d . . . . .
O16 O 0.3896(4) 0.6350(3) 0.7712(5) 0.029(2) Uani 1 1 d . . . . .
O17 O 0.3770(4) 0.6627(3) 0.8874(5) 0.028(2) Uani 1 1 d . . . . .
O18 O 0.3043(3) 0.6008(3) 0.7531(5) 0.024(2) Uani 1 1 d . . . . .
O19 O 0.3445(4) 0.4753(3) 0.6880(6) 0.042(3) Uani 1 1 d . . . . .
O20 O 0.3309(4) 0.5744(3) 0.6565(5) 0.030(2) Uani 1 1 d . . . . .
O21 O 0.2491(4) 0.5262(3) 0.6333(5) 0.035(2) Uani 1 1 d . . . . .
O22 O 0.3499(4) 0.6636(4) 0.6214(5) 0.039(3) Uani 1 1 d . . . . .
O23 O 0.2516(3) 0.6363(3) 0.5997(5) 0.027(2) Uani 1 1 d . . . . .
O24 O 0.3104(4) 0.6997(3) 0.7073(5) 0.030(2) Uani 1 1 d . . . . .
O25 O 0.1557(4) 0.6694(4) 0.4718(5) 0.043(3) Uani 1 1 d . . . . .
O26 O 0.1662(4) 0.5776(3) 0.5291(5) 0.031(2) Uani 1 1 d . . . . .
O27 O 0.1142(4) 0.6430(3) 0.5598(5) 0.028(2) Uani 1 1 d . . . . .
O28 O 0.1966(4) 0.7013(3) 0.6200(5) 0.026(2) Uani 1 1 d . . . . .
O29 O 0.1536(4) 0.4785(3) 0.5398(6) 0.045(3) Uani 1 1 d . . . . .
O30 O 0.1973(3) 0.6009(3) 0.6676(5) 0.024(2) Uani 1 1 d . . . . .
O31 O 0.1124(3) 0.5497(3) 0.5916(5) 0.031(2) Uani 1 1 d . . . . .
O32 O 0.0437(4) 0.6108(4) 0.5974(5) 0.042(3) Uani 1 1 d . . . . .
O33 O 0.1306(4) 0.6678(3) 0.6948(5) 0.030(2) Uani 1 1 d . . . . .
O34 O 0.3492(4) 0.7816(4) 0.6810(5) 0.038(2) Uani 1 1 d . . . . .
O35 O 0.2553(3) 0.7830(3) 0.6811(5) 0.025(2) Uani 1 1 d . . . . .
O36 O 0.3938(4) 0.7481(3) 0.8260(5) 0.030(2) Uani 1 1 d . U . . .
O37 O 0.3037(3) 0.7410(3) 0.8262(5) 0.0214(19) Uani 1 1 d . U . . .
O38 O 0.3360(4) 0.8294(3) 0.7910(5) 0.027(2) Uani 1 1 d . . . . .
O39 O 0.1631(4) 0.7837(3) 0.5372(5) 0.033(2) Uani 1 1 d . . . . .
O40 O 0.1203(3) 0.7507(3) 0.6220(4) 0.0207(19) Uani 1 1 d . . . . .
O41 O 0.2058(3) 0.7425(3) 0.7509(4) 0.0180(18) Uani 1 1 d . . . . .
O42 O 0.1734(4) 0.8304(3) 0.6657(5) 0.028(2) Uani 1 1 d . . . . .
O43 O 0.0524(4) 0.7321(4) 0.6699(5) 0.040(3) Uani 1 1 d . . . . .
O44 O 0.1439(3) 0.7214(3) 0.8124(5) 0.026(2) Uani 1 1 d . . . . .
O45 O 0.1306(3) 0.8042(3) 0.7362(5) 0.027(2) Uani 1 1 d . . . . .
O46 O 0.1426(4) 0.6678(3) 0.9291(5) 0.034(2) Uani 1 1 d . . . . .
O47 O 0.2500(3) 0.6684(3) 0.9924(5) 0.0222(19) Uani 1 1 d . . . . .
O48 O 0.2554(3) 0.7144(3) 0.8892(5) 0.0205(19) Uani 1 1 d . . . . .
O49 O 0.3613(4) 0.6635(3) 1.1021(5) 0.033(2) Uani 1 1 d . . . . .
O50 O 0.3043(3) 0.7479(3) 1.0456(4) 0.023(2) Uani 1 1 d . . . . .
O51 O 0.3666(3) 0.7173(3) 0.9965(5) 0.027(2) Uani 1 1 d . U . . .
O52 O 0.4643(4) 0.7335(4) 0.9971(5) 0.044(3) Uani 1 1 d . U . . .
O53 O 0.3824(4) 0.8079(3) 0.9329(5) 0.028(2) Uani 1 1 d . . . . .
O54 O 0.4011(4) 0.8880(3) 0.8905(6) 0.040(3) Uani 1 1 d . . . . .
O55 O 0.1073(4) 0.8849(3) 0.6703(6) 0.040(3) Uani 1 1 d . . . . .
C1 C 0.2575(5) 0.8058(4) 0.8679(7) 0.018(3) Uani 1 1 d . . . . .
H1A H 0.2275 0.8085 0.8738 0.021 Uiso 1 1 calc R . . . .
H1B H 0.2892 0.8082 0.9186 0.021 Uiso 1 1 calc R . . . .
C2 C 0.3035(5) 0.8791(5) 0.8662(7) 0.024(3) Uani 1 1 d . U . . .
H2A H 0.3101 0.8845 0.9171 0.029 Uiso 1 1 calc R . . . .
H2B H 0.2977 0.9103 0.8413 0.029 Uiso 1 1 calc R . . . .
C3 C 0.2047(5) 0.8778(5) 0.7918(8) 0.025(3) Uani 1 1 d . U . . .
H3A H 0.2090 0.9100 0.7771 0.030 Uiso 1 1 calc R . . . .
H3B H 0.1976 0.8811 0.8324 0.030 Uiso 1 1 calc R . . . .
O1W O 0.7495(6) 0.9522(6) 0.9850(9) 0.092(5) Uiso 1 1 d . . . . .
O2W O 0.8326(6) 0.8942(5) 0.9661(8) 0.080(4) Uiso 1 1 d . . . . .
O3W O 0.0000 0.9078(5) 0.7500 0.032(3) Uiso 1 2 d S T P . .
O4W O 0.0397(6) 0.5356(5) 0.0072(8) 0.080(4) Uiso 1 1 d . . . . .
O5W O 0.6272(6) 0.9575(5) 0.8801(9) 0.098(5) Uiso 1 1 d D . . . .
O6W O 0.0345(6) 0.7263(6) 0.4663(9) 0.095(5) Uiso 1 1 d . . . . .
O7W O 0.2484(8) 0.6709(8) 0.4568(12) 0.053(6) Uiso 0.6 1 d . . . A 1
O8W O 0.2492(12) 0.6477(12) 0.4410(18) 0.051(8) Uiso 0.4 1 d . . . B 2
O9W O 0.9934(9) 0.8531(7) 0.9346(12) 0.050(6) Uiso 0.5 1 d . . . . .
O10W O 0.6648(9) 0.8879(7) 0.8356(13) 0.055(6) Uiso 0.5 1 d D . . . .
O11W O 0.0479(9) 0.7542(7) 0.8235(12) 0.046(5) Uiso 0.5 1 d . . . . .
O12W O 0.0923(9) 0.5362(8) 0.1913(13) 0.052(6) Uiso 0.5 1 d . . . . .
O13W O 0.0938(8) 0.0384(7) 0.0745(11) 0.037(5) Uiso 0.5 1 d . . . . .
O14W O 0.8845(9) 0.9518(8) 1.0828(13) 0.054(6) Uiso 0.5 1 d . . . . .
O15W O 0.4672(11) 0.7211(10) 0.7857(16) 0.080(8) Uiso 0.5 1 d . . . . .
O16W O 0.4879(12) 0.8594(10) 0.8863(17) 0.086(9) Uiso 0.5 1 d . . . . .
O17W O 0.0659(8) 0.5842(7) -0.0828(11) 0.040(5) Uiso 0.5 1 d . . . . .
O18W O -0.0788(6) 0.9117(6) 0.7049(9) 0.095(5) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.726(9) . ?
W1 O2 1.912(9) . ?
W1 O3 1.962(9) . ?
W1 O4 1.819(8) . ?
W1 O5 1.919(8) . ?
W1 O6 2.324(8) . ?
W2 O2 1.948(9) . ?
W2 O6 2.332(8) . ?
W2 O7 1.710(9) . ?
W2 O8 1.998(9) . ?
W2 O9 1.897(9) . ?
W2 O10 1.830(8) . ?
W3 O3 1.904(9) . ?
W3 O6 2.422(8) . ?
W3 O8 1.865(9) . ?
W3 O11 1.730(8) . ?
W3 O12 1.951(9) . ?
W3 O13 1.914(9) . ?
W4 O9 1.913(9) . ?
W4 O14 1.719(9) . ?
W4 O15 2.087(9) . ?
W4 O16 1.971(9) . ?
W4 O17 1.750(9) . ?
W4 O18 2.326(9) . ?
W5 O13 1.893(9) . ?
W5 O15 1.810(9) . ?
W5 O18 2.431(8) . ?
W5 O19 1.704(9) . ?
W5 O20 1.941(9) . ?
W5 O21 1.958(10) . ?
W6 O16 1.891(9) . ?
W6 O18 2.330(8) . ?
W6 O20 1.908(9) . ?
W6 O22 1.710(9) . ?
W6 O23 1.922(9) . ?
W6 O24 1.898(9) . ?
W7 O23 1.894(9) . ?
W7 O25 1.702(9) . ?
W7 O26 1.867(9) . ?
W7 O27 1.927(9) . ?
W7 O28 1.952(8) . ?
W7 O30 2.319(8) . ?
W8 O12 1.868(8) . ?
W8 O21 1.860(10) . ?
W8 O26 1.966(9) . ?
W8 O29 1.698(9) . ?
W8 O30 2.377(8) . ?
W8 O31 1.972(9) . ?
W9 O5 1.895(8) . ?
W9 O27 1.933(9) . ?
W9 O30 2.342(9) . ?
W9 O31 1.874(9) . ?
W9 O32 1.696(10) . ?
W9 O33 1.948(8) . ?
W10 O24 1.887(9) . ?
W10 O34 1.700(9) . ?
W10 O35 2.014(9) . ?
W10 O36 1.773(9) . ?
W10 O37 2.354(8) . ?
W10 O38 2.044(8) . ?
W11 O28 1.823(8) . ?
W11 O35 1.832(9) . ?
W11 O39 1.699(8) . ?
W11 O40 1.925(8) . ?
W11 O41 2.353(8) . ?
W11 O42 2.066(9) . ?
W12 O33 1.843(9) . ?
W12 O40 1.900(8) . ?
W12 O41 2.274(8) . ?
W12 O43 1.706(9) . ?
W12 O44 1.858(8) . ?
W12 O45 2.070(9) . ?
W13 O4 1.990(8) . ?
W13 O44 1.936(8) . ?
W13 O46 1.700(9) . ?
W13 O47 1.823(8) . ?
W13 O48 2.385(8) . ?
W13 O50 1.869(8) 7_567 ?
W14 O10 1.965(8) . ?
W14 O47 2.032(8) . ?
W14 O48 2.375(8) . ?
W14 O49 1.700(9) . ?
W14 O50 1.928(8) . ?
W14 O51 1.741(9) . ?
As1 O6 1.783(8) . ?
As1 O18 1.789(8) . ?
As1 O30 1.809(8) . ?
Co1 K1 3.746(5) 7_567 ?
Co1 O17 2.031(9) . ?
Co1 O36 2.094(9) . ?
Co1 O37 2.170(8) . ?
Co1 O51 2.018(9) . ?
Co1 O52 2.023(10) . ?
Co1 O53 2.088(9) . ?
P1 O37 1.481(9) . ?
P1 O41 1.530(8) . ?
P1 O48 1.507(8) . ?
P1 C1 1.804(11) . ?
P2 K1 3.809(5) 7_567 ?
P2 O38 1.543(9) . ?
P2 O53 1.533(9) . ?
P2 O54 1.495(9) . ?
P2 C2 1.869(14) . ?
P3 O42 1.509(9) . ?
P3 O45 1.536(9) . ?
P3 O55 1.480(10) . ?
P3 C3 1.830(14) . ?
K1 Co1 3.746(5) 7_567 ?
K1 P2 3.809(5) 7_567 ?
K1 O32 3.139(12) 2_556 ?
K1 O43 2.808(10) 2_556 ?
K1 O46 2.857(10) . ?
K1 O52 3.048(11) 7_567 ?
K1 O53 2.721(10) 7_567 ?
K1 O11W 2.83(2) . ?
K1 O17W 2.76(2) 1_556 ?
K2 O22 2.940(12) 7_566 ?
K2 O25 3.084(13) . ?
K2 O34 2.989(12) 7_566 ?
K2 O39 2.925(12) . ?
K2 O6W 3.035(17) . ?
K2 O15W 2.95(3) 7_566 ?
K2 O15W 3.06(3) 8_465 ?
N1 C1 1.504(14) . ?
N1 C2 1.474(16) . ?
N1 C3 1.550(15) . ?
O22 K2 2.940(12) 7_566 ?
O32 K1 3.139(11) 2_556 ?
O34 K2 2.989(12) 7_566 ?
O43 K1 2.808(10) 2_556 ?
O50 W13 1.869(8) 7_567 ?
O52 K1 3.048(11) 7_567 ?
O53 K1 2.721(10) 7_567 ?
C1 H1A 0.9700 . ?
C1 H1B 0.9700 . ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
O15W K2 2.95(3) 7_566 ?
O15W K2 3.06(3) 8_566 ?
O17W K1 2.76(2) 1_554 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O2 99.9(4) . . ?
O1 W1 O3 95.3(4) . . ?
O1 W1 O4 102.5(4) . . ?
O1 W1 O5 101.2(4) . . ?
O1 W1 O6 168.2(4) . . ?
O2 W1 O3 85.3(4) . . ?
O2 W1 O5 158.0(4) . . ?
O2 W1 O6 73.6(3) . . ?
O3 W1 O6 74.6(3) . . ?
O4 W1 O2 92.7(4) . . ?
O4 W1 O3 162.1(4) . . ?
O4 W1 O5 88.9(4) . . ?
O4 W1 O6 87.8(3) . . ?
O5 W1 O3 86.5(4) . . ?
O5 W1 O6 84.6(3) . . ?
O2 W2 O6 72.8(3) . . ?
O2 W2 O8 83.5(4) . . ?
O7 W2 O2 99.7(4) . . ?
O7 W2 O6 167.2(4) . . ?
O7 W2 O8 95.2(4) . . ?
O7 W2 O9 102.6(4) . . ?
O7 W2 O10 101.5(4) . . ?
O8 W2 O6 73.9(3) . . ?
O9 W2 O2 156.6(4) . . ?
O9 W2 O6 83.9(3) . . ?
O9 W2 O8 87.4(4) . . ?
O10 W2 O2 91.4(4) . . ?
O10 W2 O6 89.2(3) . . ?
O10 W2 O8 163.1(4) . . ?
O10 W2 O9 91.1(4) . . ?
O3 W3 O6 73.2(3) . . ?
O3 W3 O12 85.8(4) . . ?
O3 W3 O13 157.0(4) . . ?
O8 W3 O3 91.5(4) . . ?
O8 W3 O6 74.0(3) . . ?
O8 W3 O12 159.3(4) . . ?
O8 W3 O13 90.0(4) . . ?
O11 W3 O3 101.1(4) . . ?
O11 W3 O6 171.5(4) . . ?
O11 W3 O8 100.2(4) . . ?
O11 W3 O12 100.5(4) . . ?
O11 W3 O13 101.2(4) . . ?
O12 W3 O6 85.6(3) . . ?
O13 W3 O6 85.2(3) . . ?
O13 W3 O12 84.7(4) . . ?
O9 W4 O15 84.8(4) . . ?
O9 W4 O16 155.1(4) . . ?
O9 W4 O18 83.6(3) . . ?
O14 W4 O9 101.6(4) . . ?
O14 W4 O15 92.4(4) . . ?
O14 W4 O16 99.7(4) . . ?
O14 W4 O17 103.0(5) . . ?
O14 W4 O18 162.6(4) . . ?
O15 W4 O18 71.4(3) . . ?
O16 W4 O15 81.7(4) . . ?
O16 W4 O18 72.4(3) . . ?
O17 W4 O9 93.5(4) . . ?
O17 W4 O15 164.5(4) . . ?
O17 W4 O16 94.0(4) . . ?
O17 W4 O18 93.1(4) . . ?
O13 W5 O18 85.7(3) . . ?
O13 W5 O20 155.7(4) . . ?
O13 W5 O21 84.1(4) . . ?
O15 W5 O13 91.8(4) . . ?
O15 W5 O18 73.4(3) . . ?
O15 W5 O20 91.8(4) . . ?
O15 W5 O21 157.2(4) . . ?
O19 W5 O13 102.7(4) . . ?
O19 W5 O15 102.3(5) . . ?
O19 W5 O18 170.8(4) . . ?
O19 W5 O20 99.9(4) . . ?
O19 W5 O21 100.4(5) . . ?
O20 W5 O18 72.4(3) . . ?
O20 W5 O21 83.4(4) . . ?
O21 W5 O18 83.9(3) . . ?
O16 W6 O18 73.6(3) . . ?
O16 W6 O20 88.7(4) . . ?
O16 W6 O23 157.4(4) . . ?
O16 W6 O24 90.2(4) . . ?
O20 W6 O18 75.3(3) . . ?
O20 W6 O23 87.0(4) . . ?
O22 W6 O16 100.5(4) . . ?
O22 W6 O18 170.2(4) . . ?
O22 W6 O20 97.0(4) . . ?
O22 W6 O23 102.1(4) . . ?
O22 W6 O24 100.9(4) . . ?
O23 W6 O18 83.8(3) . . ?
O24 W6 O18 87.1(3) . . ?
O24 W6 O20 161.9(4) . . ?
O24 W6 O23 87.1(4) . . ?
O23 W7 O27 156.0(4) . . ?
O23 W7 O28 85.6(4) . . ?
O23 W7 O30 83.6(3) . . ?
O25 W7 O23 103.2(4) . . ?
O25 W7 O26 100.4(5) . . ?
O25 W7 O27 100.1(4) . . ?
O25 W7 O28 97.9(4) . . ?
O25 W7 O30 172.1(4) . . ?
O26 W7 O23 91.9(4) . . ?
O26 W7 O27 89.5(4) . . ?
O26 W7 O28 161.5(4) . . ?
O26 W7 O30 75.0(3) . . ?
O27 W7 O28 85.6(4) . . ?
O27 W7 O30 73.7(3) . . ?
O28 W7 O30 86.6(3) . . ?
O12 W8 O26 158.3(4) . . ?
O12 W8 O30 86.4(3) . . ?
O12 W8 O31 87.7(4) . . ?
O21 W8 O12 90.8(4) . . ?
O21 W8 O26 88.3(4) . . ?
O21 W8 O30 84.9(3) . . ?
O21 W8 O31 157.0(4) . . ?
O26 W8 O30 71.9(3) . . ?
O26 W8 O31 84.7(4) . . ?
O29 W8 O12 102.4(4) . . ?
O29 W8 O21 102.8(5) . . ?
O29 W8 O26 98.9(4) . . ?
O29 W8 O30 168.1(4) . . ?
O29 W8 O31 100.0(5) . . ?
O31 W8 O30 72.1(3) . . ?
O5 W9 O27 156.2(4) . . ?
O5 W9 O30 84.2(3) . . ?
O5 W9 O33 86.1(4) . . ?
O27 W9 O30 73.0(3) . . ?
O27 W9 O33 86.0(3) . . ?
O31 W9 O5 91.8(4) . . ?
O31 W9 O27 88.9(4) . . ?
O31 W9 O30 74.5(3) . . ?
O31 W9 O33 162.1(4) . . ?
O32 W9 O5 105.0(4) . . ?
O32 W9 O27 98.4(4) . . ?
O32 W9 O30 168.9(4) . . ?
O32 W9 O31 98.7(4) . . ?
O32 W9 O33 99.0(4) . . ?
O33 W9 O30 87.6(3) . . ?
O24 W10 O35 88.1(4) . . ?
O24 W10 O37 82.2(3) . . ?
O24 W10 O38 160.6(4) . . ?
O34 W10 O24 98.9(4) . . ?
O34 W10 O35 97.9(4) . . ?
O34 W10 O36 102.4(4) . . ?
O34 W10 O37 176.7(4) . . ?
O34 W10 O38 97.7(4) . . ?
O35 W10 O37 78.9(3) . . ?
O35 W10 O38 79.8(3) . . ?
O36 W10 O24 96.9(4) . . ?
O36 W10 O35 158.0(4) . . ?
O36 W10 O37 80.5(3) . . ?
O36 W10 O38 89.2(4) . . ?
O38 W10 O37 80.7(3) . . ?
O28 W11 O35 96.2(4) . . ?
O28 W11 O40 91.2(4) . . ?
O28 W11 O41 83.5(3) . . ?
O28 W11 O42 163.1(4) . . ?
O35 W11 O40 152.3(3) . . ?
O35 W11 O41 82.6(3) . . ?
O35 W11 O42 85.1(4) . . ?
O39 W11 O28 99.9(4) . . ?
O39 W11 O35 103.4(4) . . ?
O39 W11 O40 101.5(4) . . ?
O39 W11 O41 172.7(4) . . ?
O39 W11 O42 96.2(4) . . ?
O40 W11 O41 71.8(3) . . ?
O40 W11 O42 80.4(4) . . ?
O42 W11 O41 80.0(3) . . ?
O33 W12 O40 90.8(4) . . ?
O33 W12 O41 85.3(3) . . ?
O33 W12 O44 93.0(4) . . ?
O33 W12 O45 162.2(4) . . ?
O40 W12 O41 74.1(3) . . ?
O40 W12 O45 83.9(3) . . ?
O43 W12 O33 101.9(5) . . ?
O43 W12 O40 98.6(4) . . ?
O43 W12 O41 169.9(4) . . ?
O43 W12 O44 101.6(4) . . ?
O43 W12 O45 95.7(4) . . ?
O44 W12 O40 158.2(4) . . ?
O44 W12 O41 84.8(3) . . ?
O44 W12 O45 86.0(4) . . ?
O45 W12 O41 76.9(3) . . ?
O4 W13 O48 79.5(3) . . ?
O44 W13 O4 84.5(3) . . ?
O44 W13 O48 81.2(3) . . ?
O46 W13 O4 95.9(4) . . ?
O46 W13 O44 102.7(4) . . ?
O46 W13 O47 102.3(4) . . ?
O46 W13 O48 173.8(4) . . ?
O46 W13 O50 98.6(4) . 7_567 ?
O47 W13 O4 88.7(3) . . ?
O47 W13 O44 154.6(4) . . ?
O47 W13 O48 73.5(3) . . ?
O47 W13 O50 93.5(4) . 7_567 ?
O50 W13 O4 164.5(4) 7_567 . ?
O50 W13 O44 87.0(4) 7_567 . ?
O50 W13 O48 86.4(3) 7_567 . ?
O10 W14 O47 83.9(3) . . ?
O10 W14 O48 78.7(3) . . ?
O47 W14 O48 70.4(3) . . ?
O49 W14 O10 97.0(4) . . ?
O49 W14 O47 99.7(4) . . ?
O49 W14 O48 169.5(4) . . ?
O49 W14 O50 98.7(4) . . ?
O49 W14 O51 103.9(4) . . ?
O50 W14 O10 160.5(4) . . ?
O50 W14 O47 82.1(3) . . ?
O50 W14 O48 83.9(3) . . ?
O51 W14 O10 93.5(4) . . ?
O51 W14 O47 156.5(4) . . ?
O51 W14 O48 86.1(4) . . ?
O51 W14 O50 94.0(4) . . ?
O6 As1 O18 97.1(4) . . ?
O6 As1 O30 97.4(4) . . ?
O18 As1 O30 97.6(4) . . ?
O17 Co1 K1 144.2(3) . 7_567 ?
O17 Co1 O36 87.3(4) . . ?
O17 Co1 O37 85.4(3) . . ?
O17 Co1 O53 170.1(4) . . ?
O36 Co1 K1 115.2(3) . 7_567 ?
O36 Co1 O37 78.7(3) . . ?
O37 Co1 K1 124.6(2) . 7_567 ?
O51 Co1 K1 71.2(3) . 7_567 ?
O51 Co1 O17 89.9(3) . . ?
O51 Co1 O36 171.6(4) . . ?
O51 Co1 O37 93.2(3) . . ?
O51 Co1 O52 93.8(4) . . ?
O51 Co1 O53 93.0(3) . . ?
O52 Co1 K1 54.3(3) . 7_567 ?
O52 Co1 O17 98.7(4) . . ?
O52 Co1 O36 94.5(4) . . ?
O52 Co1 O37 171.9(4) . . ?
O52 Co1 O53 90.5(4) . . ?
O53 Co1 K1 45.4(3) . 7_567 ?
O53 Co1 O36 88.5(3) . . ?
O53 Co1 O37 85.0(3) . . ?
O37 P1 O41 110.6(5) . . ?
O37 P1 O48 114.5(5) . . ?
O37 P1 C1 108.2(5) . . ?
O41 P1 C1 108.0(5) . . ?
O48 P1 O41 113.3(5) . . ?
O48 P1 C1 101.6(5) . . ?
O38 P2 K1 144.6(4) . 7_567 ?
O38 P2 C2 99.6(5) . . ?
O53 P2 K1 36.0(3) . 7_567 ?
O53 P2 O38 112.2(5) . . ?
O53 P2 C2 110.7(5) . . ?
O54 P2 K1 83.0(4) . 7_567 ?
O54 P2 O38 112.3(6) . . ?
O54 P2 O53 114.8(6) . . ?
O54 P2 C2 106.0(6) . . ?
C2 P2 K1 106.6(4) . 7_567 ?
O42 P3 O45 110.3(5) . . ?
O42 P3 C3 102.0(6) . . ?
O45 P3 C3 110.2(5) . . ?
O55 P3 O42 115.3(5) . . ?
O55 P3 O45 112.5(6) . . ?
O55 P3 C3 105.8(6) . . ?
Co1 K1 P2 51.62(8) 7_567 7_567 ?
O32 K1 Co1 120.6(2) 2_556 7_567 ?
O32 K1 P2 92.4(2) 2_556 7_567 ?
O43 K1 Co1 98.6(2) 2_556 7_567 ?
O43 K1 P2 135.7(3) 2_556 7_567 ?
O43 K1 O32 74.9(3) 2_556 2_556 ?
O43 K1 O46 141.6(3) 2_556 . ?
O43 K1 O52 67.2(3) 2_556 7_567 ?
O43 K1 O11W 67.6(5) 2_556 . ?
O46 K1 Co1 86.4(2) . 7_567 ?
O46 K1 P2 75.9(2) . 7_567 ?
O46 K1 O32 134.3(3) . 2_556 ?
O46 K1 O52 116.3(3) . 7_567 ?
O52 K1 Co1 32.63(19) 7_567 7_567 ?
O52 K1 P2 74.8(2) 7_567 7_567 ?
O52 K1 O32 102.2(3) 7_567 2_556 ?
O53 K1 Co1 33.11(19) 7_567 7_567 ?
O53 K1 P2 19.32(19) 7_567 7_567 ?
O53 K1 O32 107.4(3) 7_567 2_556 ?
O53 K1 O43 127.0(3) 7_567 2_556 ?
O53 K1 O46 74.4(3) 7_567 . ?
O53 K1 O52 60.5(3) 7_567 7_567 ?
O53 K1 O11W 112.9(5) 7_567 . ?
O53 K1 O17W 92.7(5) 7_567 1_556 ?
O11W K1 Co1 87.4(5) . 7_567 ?
O11W K1 P2 130.5(5) . 7_567 ?
O11W K1 O32 136.1(5) . 2_556 ?
O11W K1 O46 74.7(5) . . ?
O11W K1 O52 83.7(5) . 7_567 ?
O17W K1 Co1 125.7(4) 1_556 7_567 ?
O17W K1 P2 75.3(4) 1_556 7_567 ?
O17W K1 O32 65.5(5) 1_556 2_556 ?
O17W K1 O43 131.0(5) 1_556 2_556 ?
O17W K1 O46 68.7(5) 1_556 . ?
O17W K1 O52 147.0(5) 1_556 7_567 ?
O17W K1 O11W 127.1(6) 1_556 . ?
O22 K2 O25 111.1(4) 7_566 . ?
O22 K2 O34 72.1(3) 7_566 7_566 ?
O22 K2 O6W 138.0(5) 7_566 . ?
O22 K2 O15W 112.4(6) 7_566 8_465 ?
O22 K2 O15W 77.7(6) 7_566 7_566 ?
O34 K2 O25 67.2(3) 7_566 . ?
O34 K2 O6W 142.7(5) 7_566 . ?
O34 K2 O15W 127.0(6) 7_566 8_465 ?
O39 K2 O22 71.1(3) . 7_566 ?
O39 K2 O25 68.7(3) . . ?
O39 K2 O34 104.6(4) . 7_566 ?
O39 K2 O6W 75.8(4) . . ?
O39 K2 O15W 127.4(6) . 8_465 ?
O39 K2 O15W 148.2(6) . 7_566 ?
O6W K2 O25 79.0(4) . . ?
O6W K2 O15W 69.4(6) . 8_465 ?
O15W K2 O25 130.8(6) 7_566 . ?
O15W K2 O25 136.4(6) 8_465 . ?
O15W K2 O34 70.6(6) 7_566 7_566 ?
O15W K2 O6W 127.6(7) 7_566 . ?
O15W K2 O15W 60.1(9) 7_566 8_465 ?
C1 N1 C3 110.2(9) . . ?
C2 N1 C1 111.3(9) . . ?
C2 N1 C3 111.4(9) . . ?
W1 O2 W2 120.9(4) . . ?
W3 O3 W1 121.4(5) . . ?
W1 O4 W13 145.0(5) . . ?
W9 O5 W1 154.8(5) . . ?
W1 O6 W2 92.3(3) . . ?
W1 O6 W3 90.6(3) . . ?
W2 O6 W3 90.4(3) . . ?
As1 O6 W1 118.9(4) . . ?
As1 O6 W2 120.1(4) . . ?
As1 O6 W3 134.0(4) . . ?
W3 O8 W2 121.7(4) . . ?
W2 O9 W4 149.2(5) . . ?
W2 O10 W14 149.7(5) . . ?
W8 O12 W3 147.8(5) . . ?
W5 O13 W3 155.1(5) . . ?
W5 O15 W4 123.0(4) . . ?
W6 O16 W4 121.2(5) . . ?
W4 O17 Co1 159.1(5) . . ?
W4 O18 W5 92.2(3) . . ?
W4 O18 W6 92.5(3) . . ?
W6 O18 W5 89.9(3) . . ?
As1 O18 W4 118.9(4) . . ?
As1 O18 W5 133.3(4) . . ?
As1 O18 W6 119.9(4) . . ?
W6 O20 W5 121.9(4) . . ?
W8 O21 W5 149.6(5) . . ?
W6 O22 K2 140.3(5) . 7_566 ?
W7 O23 W6 157.6(5) . . ?
W10 O24 W6 146.7(5) . . ?
W7 O25 K2 138.4(5) . . ?
W7 O26 W8 122.0(5) . . ?
W7 O27 W9 120.8(5) . . ?
W11 O28 W7 149.8(5) . . ?
W7 O30 W8 91.1(3) . . ?
W7 O30 W9 92.1(3) . . ?
W9 O30 W8 91.1(3) . . ?
As1 O30 W7 119.5(4) . . ?
As1 O30 W8 133.7(4) . . ?
As1 O30 W9 118.9(4) . . ?
W9 O31 W8 122.3(4) . . ?
W9 O32 K1 140.8(5) . 2_556 ?
W12 O33 W9 152.8(5) . . ?
W10 O34 K2 137.4(5) . 7_566 ?
W11 O35 W10 148.8(5) . . ?
W10 O36 Co1 110.7(4) . . ?
Co1 O37 W10 89.5(3) . . ?
P1 O37 W10 138.2(5) . . ?
P1 O37 Co1 128.8(5) . . ?
P2 O38 W10 134.9(5) . . ?
W11 O39 K2 140.1(5) . . ?
W12 O40 W11 121.7(4) . . ?
W12 O41 W11 92.4(3) . . ?
P1 O41 W11 132.9(5) . . ?
P1 O41 W12 133.1(5) . . ?
P3 O42 W11 137.4(5) . . ?
W12 O43 K1 146.3(6) . 2_556 ?
W12 O44 W13 154.4(5) . . ?
P3 O45 W12 134.8(5) . . ?
W13 O46 K1 146.6(5) . . ?
W13 O47 W14 123.4(4) . . ?
W14 O48 W13 91.0(3) . . ?
P1 O48 W13 133.5(5) . . ?
P1 O48 W14 133.1(5) . . ?
W13 O50 W14 159.6(5) 7_567 . ?
W14 O51 Co1 146.9(5) . . ?
Co1 O52 K1 93.0(4) . 7_567 ?
Co1 O53 K1 101.5(3) . 7_567 ?
P2 O53 Co1 130.0(5) . . ?
P2 O53 K1 124.7(5) . 7_567 ?
P1 C1 H1A 108.0 . . ?
P1 C1 H1B 108.0 . . ?
N1 C1 P1 117.1(8) . . ?
N1 C1 H1A 108.0 . . ?
N1 C1 H1B 108.0 . . ?
H1A C1 H1B 107.3 . . ?
P2 C2 H2A 109.8 . . ?
P2 C2 H2B 109.8 . . ?
N1 C2 P2 109.6(8) . . ?
N1 C2 H2A 109.8 . . ?
N1 C2 H2B 109.8 . . ?
H2A C2 H2B 108.2 . . ?
P3 C3 H3A 109.5 . . ?
P3 C3 H3B 109.5 . . ?
N1 C3 P3 110.5(8) . . ?
N1 C3 H3A 109.5 . . ?
N1 C3 H3B 109.5 . . ?
H3A C3 H3B 108.1 . . ?
K2 O15W K2 114.2(9) 7_566 8_566 ?

_shelx_SHELXL_version_number     2014/7
_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_3
_database_code_depnum_ccdc_archive 'CCDC 987934'
_audit_update_record             
;
2015-11-22 deposited with the CCDC.
2015-11-30 downloaded from the CCDC.
;
_audit_creation_date             2015-11-21
_audit_creation_method           
;
Olex2 1.2
(compiled 2015.09.30 svn.r3233 for OlexSys, GUI svn.r5103)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         
'0.5(C12 H16 As4 K8 Mn4 N4 O232 P12 W56), 18(O)'
_chemical_formula_sum            'C6 H74 As2 K4 Mn2 N2 O134 P6 W28'
_chemical_formula_weight         8068.06
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 1 2/c 1'
_space_group_name_Hall           '-C 2yc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   29.848(4)
_cell_length_b                   27.794(4)
_cell_length_c                   20.700(3)
_cell_angle_alpha                90
_cell_angle_beta                 121.555(2)
_cell_angle_gamma                90
_cell_volume                     14634(4)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    4537
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      26.16
_cell_measurement_theta_min      2.48
_shelx_estimated_absorpt_T_max   0.131
_shelx_estimated_absorpt_T_min   0.031
_exptl_absorpt_coefficient_mu    22.809
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.2102
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2008/1 (Bruker,2008) was used for absorption correction.
wR2(int) was 0.1654 before and 0.0652 after correction.
The Ratio of minimum to maximum transmission is 0.2819.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.657
_exptl_crystal_density_meas      .
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             14152
_exptl_crystal_size_max          0.5
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.15
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.1079
_diffrn_reflns_av_unetI/netI     0.1297
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -35
_diffrn_reflns_limit_k_max       33
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            37013
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.866
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                7201
_reflns_number_total             12968
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         5.201
_refine_diff_density_min         -2.377
_refine_diff_density_rms         0.570
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.956
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     785
_refine_ls_number_reflns         12968
_refine_ls_number_restraints     79
_refine_ls_R_factor_all          0.1457
_refine_ls_R_factor_gt           0.0691
_refine_ls_restrained_S_all      0.955
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0937P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1578
_refine_ls_wR_factor_ref         0.1847
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H,H) groups
2. Restrained distances
 O4W-O9W
 2.7 with sigma of 0.02
3. Rigid bond restraints
 N1, C3
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 P2, C2
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 Mn1, O36
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 Mn1, O37
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 Mn1, O51
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 Mn1, O52
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
4. Uiso/Uaniso restraints and constraints
Uanis(Mn1) \\sim Ueq: with sigma of 0.001 and sigma for terminal atoms of 0.002
Uanis(C3) \\sim Ueq, Uanis(C2) \\sim Ueq, Uanis(O4) \\sim Ueq, Uanis(O35) \\sim
Ueq, Uanis(O11) \\sim Ueq, Uanis(O21) \\sim Ueq, Uanis(O39) \\sim Ueq,
Uanis(O47) \\sim Ueq, Uanis(C1) \\sim Ueq, Uanis(O22) \\sim Ueq, Uanis(O52)
\\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
5. Others
 Fixed Sof: O7W(0.6) O8W(0.4) O10W(0.5) O11W(0.5) O12W(0.5) O14W(0.5)
 O15W(0.5) O16W(0.5)
6.a Secondary CH2 refined with riding coordinates:
 C1(H1A,H1B), C3(H3A,H3B)
;
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.18332(5) 0.56948(3) 0.84347(6) 0.0309(3) Uani 1 1 d . . . . .
W2 W 0.31560(5) 0.56573(3) 0.94442(6) 0.0308(3) Uani 1 1 d . . . . .
W3 W 0.24726(5) 0.48560(3) 0.80292(6) 0.0353(3) Uani 1 1 d . . . . .
W4 W 0.38978(5) 0.60589(4) 0.85757(6) 0.0332(3) Uani 1 1 d . . . . .
W5 W 0.32327(5) 0.52348(4) 0.71522(6) 0.0352(3) Uani 1 1 d . . . . .
W6 W 0.32611(5) 0.64045(3) 0.67412(6) 0.0314(3) Uani 1 1 d . . . . .
W7 W 0.17923(5) 0.64199(3) 0.56059(6) 0.0304(3) Uani 1 1 d . . . . .
W8 W 0.17850(5) 0.52546(4) 0.60429(6) 0.0355(3) Uani 1 1 d . . . . .
W9 W 0.11133(5) 0.60767(4) 0.64117(6) 0.0331(3) Uani 1 1 d . . . . .
W10 W 0.33129(5) 0.76243(4) 0.74171(6) 0.0341(3) Uani 1 1 d . . . . .
W11 W 0.18568(5) 0.76456(3) 0.62911(6) 0.0320(3) Uani 1 1 d . . . . .
W12 W 0.11998(5) 0.73142(4) 0.71163(6) 0.0334(3) Uani 1 1 d . . . . .
W13 W 0.18727(5) 0.69133(3) 0.91160(5) 0.0272(3) Uani 1 1 d . . . . .
W14 W 0.32085(5) 0.68821(3) 1.01357(5) 0.0286(3) Uani 1 1 d . . . . .
As1 As 0.25098(11) 0.62109(8) 0.76057(13) 0.0221(6) Uani 1 1 d . . . . .
Mn1 Mn 0.38816(13) 0.73270(10) 0.91983(15) 0.0062(6) Uani 1 1 d . U . . .
P1 P 0.2558(3) 0.7460(2) 0.8294(3) 0.0224(16) Uani 1 1 d . . . . .
P2 P 0.3613(3) 0.8495(2) 0.8695(4) 0.0377(19) Uani 1 1 d . U . . .
P3 P 0.1489(3) 0.8474(2) 0.7097(4) 0.0360(19) Uani 1 1 d . . . . .
K1 K 0.0411(5) 0.6790(4) 0.9153(5) 0.105(4) Uani 1 1 d . . . . .
K2 K 0.0880(7) 0.7534(5) 0.3824(7) 0.164(6) Uani 1 1 d . . . . .
N1 N 0.2558(8) 0.8482(6) 0.8192(10) 0.021(4) Uani 1 1 d . U . . .
O1 O 0.1397(8) 0.5546(6) 0.8701(10) 0.043(5) Uani 1 1 d . . . . .
O2 O 0.2495(8) 0.5605(5) 0.9387(10) 0.035(5) Uani 1 1 d . . . . .
O3 O 0.1926(8) 0.5025(5) 0.8215(9) 0.038(5) Uani 1 1 d . . . . .
O4 O 0.1862(7) 0.6346(5) 0.8507(9) 0.025(4) Uani 1 1 d . U . . .
O5 O 0.1361(7) 0.5753(6) 0.7348(9) 0.033(5) Uani 1 1 d . . . . .
O6 O 0.2503(7) 0.5720(5) 0.8154(8) 0.024(4) Uani 1 1 d . . . . .
O7 O 0.3562(8) 0.5497(7) 1.0362(9) 0.047(6) Uani 1 1 d . . . . .
O8 O 0.2998(8) 0.4977(6) 0.9039(9) 0.039(5) Uani 1 1 d . . . . .
O9 O 0.3616(9) 0.5708(7) 0.9068(9) 0.048(6) Uani 1 1 d . . . . .
O10 O 0.3128(8) 0.6318(5) 0.9507(8) 0.033(5) Uani 1 1 d . . . . .
O11 O 0.2478(9) 0.4229(6) 0.8084(10) 0.052(6) Uani 1 1 d . U . . .
O12 O 0.1946(8) 0.4979(5) 0.6960(9) 0.034(5) Uani 1 1 d . . . . .
O13 O 0.2972(8) 0.4958(5) 0.7741(9) 0.036(5) Uani 1 1 d . . . . .
O14 O 0.4535(9) 0.6002(6) 0.9172(12) 0.056(6) Uani 1 1 d . . . . .
O15 O 0.3831(9) 0.5415(6) 0.8016(10) 0.048(6) Uani 1 1 d . . . . .
O16 O 0.3902(7) 0.6345(5) 0.7716(9) 0.030(4) Uani 1 1 d . . . . .
O17 O 0.3764(8) 0.6616(5) 0.8862(9) 0.040(5) Uani 1 1 d . . . . .
O18 O 0.3051(7) 0.5992(5) 0.7536(8) 0.030(5) Uani 1 1 d . . . . .
O19 O 0.3443(9) 0.4735(6) 0.6875(11) 0.055(6) Uani 1 1 d . . . . .
O20 O 0.3305(9) 0.5737(6) 0.6559(10) 0.050(6) Uani 1 1 d . . . . .
O21 O 0.2477(8) 0.5251(6) 0.6332(9) 0.040(5) Uani 1 1 d . U . . .
O22 O 0.3520(8) 0.6640(7) 0.6237(10) 0.044(5) Uani 1 1 d . U . . .
O23 O 0.2521(10) 0.6356(5) 0.6018(10) 0.053(7) Uani 1 1 d . . . . .
O24 O 0.3112(8) 0.6987(6) 0.7062(9) 0.039(5) Uani 1 1 d . . . . .
O25 O 0.1573(10) 0.6677(7) 0.4732(10) 0.060(7) Uani 1 1 d . . . . .
O26 O 0.1677(8) 0.5755(6) 0.5319(10) 0.043(5) Uani 1 1 d . . . . .
O27 O 0.1157(8) 0.6414(6) 0.5621(9) 0.036(5) Uani 1 1 d . . . . .
O28 O 0.1965(8) 0.7010(5) 0.6205(9) 0.039(5) Uani 1 1 d . . . . .
O29 O 0.1537(9) 0.4782(6) 0.5413(10) 0.053(6) Uani 1 1 d . . . . .
O30 O 0.1986(7) 0.6005(5) 0.6700(8) 0.026(4) Uani 1 1 d . . . . .
O31 O 0.1147(8) 0.5497(7) 0.5958(10) 0.046(5) Uani 1 1 d . . . . .
O32 O 0.0482(10) 0.6099(6) 0.6033(10) 0.060(7) Uani 1 1 d . . . . .
O33 O 0.1308(7) 0.6690(5) 0.6963(8) 0.031(5) Uani 1 1 d . . . . .
O34 O 0.3484(7) 0.7802(6) 0.6768(9) 0.035(5) Uani 1 1 d . . . . .
O35 O 0.2555(8) 0.7824(7) 0.6799(9) 0.042(5) Uani 1 1 d . U . . .
O36 O 0.3924(7) 0.7483(6) 0.8195(9) 0.032(5) Uani 1 1 d . U . . .
O37 O 0.3037(7) 0.7412(5) 0.8245(8) 0.024(4) Uani 1 1 d . U . . .
O38 O 0.3339(8) 0.8276(5) 0.7857(8) 0.035(5) Uani 1 1 d . . . . .
O39 O 0.1650(7) 0.7825(6) 0.5390(8) 0.033(4) Uani 1 1 d . U . . .
O40 O 0.1214(8) 0.7505(5) 0.6247(9) 0.039(5) Uani 1 1 d . . . . .
O41 O 0.2049(7) 0.7424(5) 0.7512(8) 0.028(4) Uani 1 1 d . . . . .
O42 O 0.1746(9) 0.8294(6) 0.6652(9) 0.044(6) Uani 1 1 d . . . . .
O43 O 0.0557(8) 0.7309(7) 0.6724(10) 0.049(6) Uani 1 1 d . . . . .
O44 O 0.1425(8) 0.7215(6) 0.8130(9) 0.038(5) Uani 1 1 d . . . . .
O45 O 0.1312(8) 0.8046(6) 0.7381(10) 0.046(5) Uani 1 1 d . . . . .
O46 O 0.1440(7) 0.6678(6) 0.9319(9) 0.032(4) Uani 1 1 d . . . . .
O47 O 0.2503(7) 0.6679(5) 0.9926(8) 0.025(4) Uani 1 1 d . U . . .
O48 O 0.2560(7) 0.7147(5) 0.8908(8) 0.024(4) Uani 1 1 d . . . . .
O49 O 0.3591(7) 0.6620(6) 1.1003(8) 0.033(5) Uani 1 1 d . . . . .
O50 O 0.3038(8) 0.7478(5) 1.0434(10) 0.044(5) Uani 1 1 d . . . . .
O51 O 0.3655(8) 0.7155(6) 0.9976(10) 0.037(5) Uani 1 1 d . U . . .
O52 O 0.4722(9) 0.7336(7) 1.0032(12) 0.061(6) Uani 1 1 d . U . . .
O53 O 0.3828(8) 0.8114(6) 0.9317(9) 0.040(5) Uani 1 1 d . . . . .
O54 O 0.4009(8) 0.8910(6) 0.8855(11) 0.054(6) Uani 1 1 d . . . . .
O55 O 0.1067(8) 0.8845(6) 0.6689(10) 0.041(5) Uani 1 1 d . . . . .
C1 C 0.2559(11) 0.8069(8) 0.8665(13) 0.029(6) Uani 1 1 d . U . . .
H1A H 0.2252 0.8098 0.8708 0.034 Uiso 1 1 calc R . . . .
H1B H 0.2867 0.8098 0.9171 0.034 Uiso 1 1 calc R . . . .
C2 C 0.3013(11) 0.8785(8) 0.8604(14) 0.030(5) Uani 1 1 d . U . . .
C3 C 0.2061(10) 0.8771(8) 0.7922(13) 0.028(6) Uani 1 1 d . U . . .
H3A H 0.2105 0.9092 0.7778 0.034 Uiso 1 1 calc R . . . .
H3B H 0.1995 0.8802 0.8332 0.034 Uiso 1 1 calc R . . . .
O1W O 0.7504(12) 0.9541(10) 0.9891(15) 0.101(9) Uiso 1 1 d . . . . .
O2W O 0.8343(12) 0.8942(10) 0.9722(15) 0.096(9) Uiso 1 1 d . . . . .
O3W O 0.0771(11) 0.9143(10) 0.8027(13) 0.090(8) Uiso 1 1 d . . . . .
O4W O 0.0394(13) 0.5371(10) 0.0117(16) 0.111(10) Uiso 1 1 d D . . . .
O5W O 0.6315(9) 0.9561(7) 0.8849(11) 0.061(6) Uiso 1 1 d . . . . .
O6W O 0.0386(16) 0.7172(13) 0.4671(19) 0.144(13) Uiso 1 1 d . . . . .
O7W O 0.2505(14) 0.6694(13) 0.4594(18) 0.049(9) Uiso 0.6 1 d . . P A 1
O8W O 0.241(3) 0.646(2) 0.429(3) 0.069(18) Uiso 0.4 1 d . . P B 2
O9W O 0.0668(12) 0.5796(10) -0.0806(15) 0.105(9) Uiso 1 1 d D . . . .
O10W O 0.6684(19) 0.8867(15) 0.847(2) 0.062(12) Uiso 0.5 1 d . . P . .
O11W O 0.0430(18) 0.7525(14) 0.818(2) 0.058(12) Uiso 0.5 1 d . . P . .
O12W O 0.0904(17) 0.5340(13) 0.190(2) 0.050(11) Uiso 0.5 1 d . . P . .
O13W O 0.0948(12) 0.0371(10) 0.0749(15) 0.099(9) Uiso 1 1 d . . . . .
O14W O 0.889(2) 0.9498(17) 1.086(3) 0.080(15) Uiso 0.5 1 d . . P . .
O15W O 0.463(2) 0.724(2) 0.787(3) 0.100(18) Uiso 0.5 1 d . . P . .
O16W O 0.486(3) 0.862(2) 0.869(3) 0.12(2) Uiso 0.5 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.708(18) . ?
W1 O2 1.944(19) . ?
W1 O3 1.969(15) . ?
W1 O4 1.813(14) . ?
W1 O5 1.937(16) . ?
W1 O6 2.357(18) . ?
W2 O2 1.919(19) . ?
W2 O6 2.348(15) . ?
W2 O7 1.693(16) . ?
W2 O8 2.022(18) . ?
W2 O9 1.91(2) . ?
W2 O10 1.846(15) . ?
W3 O3 1.920(19) . ?
W3 O6 2.412(13) . ?
W3 O8 1.874(17) . ?
W3 O11 1.745(16) . ?
W3 O12 1.961(17) . ?
W3 O13 1.894(18) . ?
W4 O9 1.894(19) . ?
W4 O14 1.65(2) . ?
W4 O15 2.083(18) . ?
W4 O16 1.955(16) . ?
W4 O17 1.777(15) . ?
W4 O18 2.316(18) . ?
W5 O13 1.918(16) . ?
W5 O15 1.82(2) . ?
W5 O18 2.410(15) . ?
W5 O19 1.740(18) . ?
W5 O20 1.944(17) . ?
W5 O21 1.99(2) . ?
W6 O16 1.928(17) . ?
W6 O18 2.343(15) . ?
W6 O20 1.910(17) . ?
W6 O22 1.720(17) . ?
W6 O23 1.92(2) . ?
W6 O24 1.888(16) . ?
W7 O23 1.88(2) . ?
W7 O25 1.725(16) . ?
W7 O26 1.917(17) . ?
W7 O27 1.91(2) . ?
W7 O28 1.955(16) . ?
W7 O30 2.327(14) . ?
W8 O12 1.863(15) . ?
W8 O21 1.83(2) . ?
W8 O26 1.944(17) . ?
W8 O29 1.722(17) . ?
W8 O30 2.389(13) . ?
W8 O31 1.94(2) . ?
W9 O5 1.901(15) . ?
W9 O27 1.950(16) . ?
W9 O30 2.357(18) . ?
W9 O31 1.893(17) . ?
W9 O32 1.62(3) . ?
W9 O33 1.964(15) . ?
W10 O24 1.892(16) . ?
W10 O34 1.741(15) . ?
W10 O35 2.01(2) . ?
W10 O36 1.733(18) . ?
W10 O37 2.332(14) . ?
W10 O38 2.011(15) . ?
W11 O28 1.822(15) . ?
W11 O35 1.85(2) . ?
W11 O39 1.703(14) . ?
W11 O40 1.91(2) . ?
W11 O41 2.363(14) . ?
W11 O42 2.043(16) . ?
W12 O33 1.821(15) . ?
W12 O40 1.898(17) . ?
W12 O41 2.240(19) . ?
W12 O43 1.65(2) . ?
W12 O44 1.858(16) . ?
W12 O45 2.087(18) . ?
W13 O4 2.009(14) . ?
W13 O44 1.949(17) . ?
W13 O46 1.686(17) . ?
W13 O47 1.864(17) . ?
W13 O48 2.398(17) . ?
W13 O50 1.883(15) 7_567 ?
W14 O10 1.970(15) . ?
W14 O47 1.997(17) . ?
W14 O48 2.367(15) . ?
W14 O49 1.706(15) . ?
W14 O50 1.926(16) . ?
W14 O51 1.711(18) . ?
As1 O6 1.782(14) . ?
As1 O18 1.801(18) . ?
As1 O30 1.794(15) . ?
Mn1 K1 3.819(10) 7_567 ?
Mn1 O17 2.063(15) . ?
Mn1 O36 2.189(15) . ?
Mn1 O37 2.258(17) . ?
Mn1 O51 2.100(16) . ?
Mn1 O52 2.18(2) . ?
Mn1 O53 2.215(17) . ?
P1 O37 1.492(17) . ?
P1 O41 1.537(17) . ?
P1 O48 1.536(15) . ?
P1 C1 1.86(2) . ?
P2 O38 1.601(16) . ?
P2 O53 1.525(17) . ?
P2 O54 1.56(2) . ?
P2 C2 1.88(3) . ?
P3 O42 1.56(2) . ?
P3 O45 1.537(19) . ?
P3 O55 1.501(19) . ?
P3 C3 1.86(3) . ?
K1 Mn1 3.819(10) 7_567 ?
K1 O32 3.14(3) 2_556 ?
K1 O43 2.87(2) 2_556 ?
K1 O46 2.92(2) . ?
K1 O52 3.10(2) 7_567 ?
K1 O53 2.780(19) 7_567 ?
K1 O9W 2.86(3) 1_556 ?
K1 O11W 2.88(4) . ?
K2 O22 2.96(2) 7_566 ?
K2 O25 3.07(3) . ?
K2 O34 2.90(2) 7_566 ?
K2 O39 2.94(2) . ?
K2 O6W 2.99(4) . ?
K2 O15W 3.07(5) 7_566 ?
K2 O15W 3.25(6) 8_465 ?
N1 C1 1.51(3) . ?
N1 C2 1.44(3) . ?
N1 C3 1.52(3) . ?
O22 K2 2.96(2) 7_566 ?
O32 K1 3.14(3) 2_556 ?
O34 K2 2.90(2) 7_566 ?
O43 K1 2.87(2) 2_556 ?
O50 W13 1.883(15) 7_567 ?
O52 K1 3.10(2) 7_567 ?
O53 K1 2.780(19) 7_567 ?
C1 H1A 0.9700 . ?
C1 H1B 0.9700 . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
O9W K1 2.86(3) 1_554 ?
O15W K2 3.07(5) 7_566 ?
O15W K2 3.25(6) 8_566 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O2 100.6(8) . . ?
O1 W1 O3 93.9(8) . . ?
O1 W1 O4 103.0(8) . . ?
O1 W1 O5 100.4(8) . . ?
O1 W1 O6 167.0(7) . . ?
O2 W1 O3 85.5(7) . . ?
O2 W1 O6 73.2(6) . . ?
O3 W1 O6 74.4(6) . . ?
O4 W1 O2 93.8(7) . . ?
O4 W1 O3 162.8(8) . . ?
O4 W1 O5 89.3(7) . . ?
O4 W1 O6 89.0(6) . . ?
O5 W1 O2 157.5(7) . . ?
O5 W1 O3 85.1(7) . . ?
O5 W1 O6 84.6(6) . . ?
O2 W2 O6 73.8(7) . . ?
O2 W2 O8 83.9(7) . . ?
O7 W2 O2 99.1(9) . . ?
O7 W2 O6 167.5(8) . . ?
O7 W2 O8 95.3(8) . . ?
O7 W2 O9 103.4(9) . . ?
O7 W2 O10 102.5(8) . . ?
O8 W2 O6 73.9(6) . . ?
O9 W2 O2 156.6(7) . . ?
O9 W2 O6 82.9(7) . . ?
O9 W2 O8 87.8(8) . . ?
O10 W2 O2 89.9(7) . . ?
O10 W2 O6 88.0(6) . . ?
O10 W2 O8 161.9(7) . . ?
O10 W2 O9 91.3(8) . . ?
O3 W3 O6 73.9(6) . . ?
O3 W3 O12 85.4(8) . . ?
O8 W3 O3 92.0(8) . . ?
O8 W3 O6 74.9(6) . . ?
O8 W3 O12 159.5(6) . . ?
O8 W3 O13 89.3(8) . . ?
O11 W3 O3 102.2(9) . . ?
O11 W3 O6 171.2(7) . . ?
O11 W3 O8 97.6(8) . . ?
O11 W3 O12 102.8(8) . . ?
O11 W3 O13 100.9(9) . . ?
O12 W3 O6 84.9(5) . . ?
O13 W3 O3 156.5(7) . . ?
O13 W3 O6 83.9(6) . . ?
O13 W3 O12 85.3(8) . . ?
O9 W4 O15 85.3(7) . . ?
O9 W4 O16 156.1(8) . . ?
O9 W4 O18 83.3(7) . . ?
O14 W4 O9 102.2(9) . . ?
O14 W4 O15 94.0(9) . . ?
O14 W4 O16 99.6(9) . . ?
O14 W4 O17 102.0(9) . . ?
O14 W4 O18 163.8(7) . . ?
O15 W4 O18 71.0(7) . . ?
O16 W4 O15 83.5(6) . . ?
O16 W4 O18 73.1(6) . . ?
O17 W4 O9 91.6(8) . . ?
O17 W4 O15 164.0(9) . . ?
O17 W4 O16 93.3(7) . . ?
O17 W4 O18 93.1(7) . . ?
O13 W5 O18 84.5(6) . . ?
O13 W5 O20 154.9(7) . . ?
O13 W5 O21 84.0(8) . . ?
O15 W5 O13 90.1(8) . . ?
O15 W5 O18 73.1(7) . . ?
O15 W5 O20 92.6(8) . . ?
O15 W5 O21 157.7(7) . . ?
O19 W5 O13 103.0(8) . . ?
O19 W5 O15 101.9(9) . . ?
O19 W5 O18 171.1(9) . . ?
O19 W5 O20 100.8(8) . . ?
O19 W5 O21 100.3(9) . . ?
O20 W5 O18 72.5(6) . . ?
O20 W5 O21 84.0(8) . . ?
O21 W5 O18 84.9(6) . . ?
O16 W6 O18 73.0(7) . . ?
O20 W6 O16 89.5(8) . . ?
O20 W6 O18 74.6(6) . . ?
O20 W6 O23 87.0(8) . . ?
O22 W6 O16 98.8(9) . . ?
O22 W6 O18 169.2(8) . . ?
O22 W6 O20 98.7(8) . . ?
O22 W6 O23 104.6(8) . . ?
O22 W6 O24 98.7(8) . . ?
O23 W6 O16 156.6(7) . . ?
O23 W6 O18 83.7(7) . . ?
O24 W6 O16 89.5(7) . . ?
O24 W6 O18 88.5(6) . . ?
O24 W6 O20 162.6(8) . . ?
O24 W6 O23 87.1(8) . . ?
O23 W7 O26 91.5(8) . . ?
O23 W7 O27 155.7(7) . . ?
O23 W7 O28 86.2(8) . . ?
O23 W7 O30 82.7(7) . . ?
O25 W7 O23 103.2(10) . . ?
O25 W7 O26 99.6(9) . . ?
O25 W7 O27 100.7(10) . . ?
O25 W7 O28 98.4(8) . . ?
O25 W7 O30 172.1(9) . . ?
O26 W7 O28 161.9(7) . . ?
O26 W7 O30 74.8(6) . . ?
O27 W7 O26 88.8(7) . . ?
O27 W7 O28 86.1(8) . . ?
O27 W7 O30 73.9(7) . . ?
O28 W7 O30 87.1(6) . . ?
O12 W8 O26 158.6(7) . . ?
O12 W8 O30 85.7(5) . . ?
O12 W8 O31 87.3(8) . . ?
O21 W8 O12 91.2(8) . . ?
O21 W8 O26 87.6(8) . . ?
O21 W8 O30 85.1(7) . . ?
O21 W8 O31 157.0(7) . . ?
O26 W8 O30 72.9(6) . . ?
O29 W8 O12 103.7(7) . . ?
O29 W8 O21 102.0(9) . . ?
O29 W8 O26 97.5(8) . . ?
O29 W8 O30 167.9(8) . . ?
O29 W8 O31 100.7(10) . . ?
O31 W8 O26 85.6(8) . . ?
O31 W8 O30 71.9(7) . . ?
O5 W9 O27 157.3(8) . . ?
O5 W9 O30 85.0(7) . . ?
O5 W9 O33 88.8(6) . . ?
O27 W9 O30 72.6(7) . . ?
O27 W9 O33 86.6(6) . . ?
O31 W9 O5 90.5(7) . . ?
O31 W9 O27 87.0(7) . . ?
O31 W9 O30 73.4(7) . . ?
O31 W9 O33 162.0(8) . . ?
O32 W9 O5 104.3(9) . . ?
O32 W9 O27 98.5(9) . . ?
O32 W9 O30 167.8(7) . . ?
O32 W9 O31 98.3(9) . . ?
O32 W9 O33 99.4(8) . . ?
O33 W9 O30 88.5(7) . . ?
O24 W10 O35 89.4(8) . . ?
O24 W10 O37 83.5(6) . . ?
O24 W10 O38 161.6(8) . . ?
O34 W10 O24 97.3(7) . . ?
O34 W10 O35 96.7(8) . . ?
O34 W10 O37 176.6(7) . . ?
O34 W10 O38 97.9(7) . . ?
O35 W10 O37 80.0(6) . . ?
O35 W10 O38 78.6(7) . . ?
O36 W10 O24 96.5(8) . . ?
O36 W10 O34 101.0(8) . . ?
O36 W10 O35 160.5(7) . . ?
O36 W10 O37 82.2(7) . . ?
O36 W10 O38 90.7(7) . . ?
O38 W10 O37 80.8(6) . . ?
O28 W11 O35 96.4(9) . . ?
O28 W11 O40 91.2(8) . . ?
O28 W11 O41 84.0(6) . . ?
O28 W11 O42 164.3(7) . . ?
O35 W11 O40 152.7(7) . . ?
O35 W11 O41 83.8(7) . . ?
O35 W11 O42 84.5(8) . . ?
O39 W11 O28 99.1(7) . . ?
O39 W11 O35 101.4(8) . . ?
O39 W11 O40 103.2(8) . . ?
O39 W11 O41 173.5(8) . . ?
O39 W11 O42 96.1(7) . . ?
O40 W11 O41 71.0(7) . . ?
O40 W11 O42 81.3(7) . . ?
O42 W11 O41 80.5(5) . . ?
O33 W12 O40 90.4(6) . . ?
O33 W12 O41 85.6(7) . . ?
O33 W12 O44 93.5(7) . . ?
O33 W12 O45 162.6(8) . . ?
O40 W12 O41 74.1(7) . . ?
O40 W12 O45 84.0(6) . . ?
O43 W12 O33 99.9(9) . . ?
O43 W12 O40 97.7(9) . . ?
O43 W12 O41 170.3(7) . . ?
O43 W12 O44 101.3(9) . . ?
O43 W12 O45 97.2(9) . . ?
O44 W12 O40 159.7(8) . . ?
O44 W12 O41 86.3(7) . . ?
O44 W12 O45 86.3(7) . . ?
O45 W12 O41 77.0(7) . . ?
O4 W13 O48 80.5(6) . . ?
O44 W13 O4 84.4(6) . . ?
O44 W13 O48 82.9(7) . . ?
O46 W13 O4 95.1(7) . . ?
O46 W13 O44 103.5(8) . . ?
O46 W13 O47 100.6(8) . . ?
O46 W13 O48 171.9(7) . . ?
O46 W13 O50 98.9(8) . 7_567 ?
O47 W13 O4 88.2(6) . . ?
O47 W13 O44 155.3(7) . . ?
O47 W13 O48 72.6(6) . . ?
O47 W13 O50 93.1(7) . 7_567 ?
O50 W13 O4 165.5(7) 7_567 . ?
O50 W13 O44 88.5(7) 7_567 . ?
O50 W13 O48 86.1(7) 7_567 . ?
O10 W14 O47 83.2(7) . . ?
O10 W14 O48 77.9(6) . . ?
O47 W14 O48 71.3(6) . . ?
O49 W14 O10 98.0(7) . . ?
O49 W14 O47 99.0(8) . . ?
O49 W14 O48 169.7(7) . . ?
O49 W14 O50 99.9(8) . . ?
O49 W14 O51 103.4(9) . . ?
O50 W14 O10 159.1(8) . . ?
O50 W14 O47 83.5(7) . . ?
O50 W14 O48 82.7(7) . . ?
O51 W14 O10 93.6(8) . . ?
O51 W14 O47 157.5(8) . . ?
O51 W14 O48 86.3(7) . . ?
O51 W14 O50 92.6(8) . . ?
O6 As1 O18 95.9(7) . . ?
O6 As1 O30 97.4(7) . . ?
O30 As1 O18 97.8(8) . . ?
O17 Mn1 K1 146.5(5) . 7_567 ?
O17 Mn1 O36 87.3(6) . . ?
O17 Mn1 O37 83.7(7) . . ?
O17 Mn1 O51 88.5(6) . . ?
O17 Mn1 O52 101.5(8) . . ?
O17 Mn1 O53 166.7(7) . . ?
O36 Mn1 K1 116.2(5) . 7_567 ?
O36 Mn1 O37 75.1(6) . . ?
O36 Mn1 O53 87.3(6) . . ?
O37 Mn1 K1 123.8(4) . 7_567 ?
O51 Mn1 K1 73.2(5) . 7_567 ?
O51 Mn1 O36 166.8(7) . . ?
O51 Mn1 O37 92.0(7) . . ?
O51 Mn1 O52 95.4(8) . . ?
O51 Mn1 O53 93.9(6) . . ?
O52 Mn1 K1 54.3(6) . 7_567 ?
O52 Mn1 O36 97.8(8) . . ?
O52 Mn1 O37 171.1(7) . . ?
O52 Mn1 O53 91.2(8) . . ?
O53 Mn1 K1 46.0(5) . 7_567 ?
O53 Mn1 O37 83.2(6) . . ?
O37 P1 O41 112.1(9) . . ?
O37 P1 O48 114.5(9) . . ?
O37 P1 C1 108.4(11) . . ?
O41 P1 C1 106.4(10) . . ?
O48 P1 O41 114.1(10) . . ?
O48 P1 C1 100.1(9) . . ?
O38 P2 C2 97.7(11) . . ?
O53 P2 O38 113.7(9) . . ?
O53 P2 O54 113.4(12) . . ?
O53 P2 C2 110.0(11) . . ?
O54 P2 O38 114.3(11) . . ?
O54 P2 C2 106.2(11) . . ?
O42 P3 C3 100.7(12) . . ?
O45 P3 O42 110.6(10) . . ?
O45 P3 C3 109.1(11) . . ?
O55 P3 O42 114.6(10) . . ?
O55 P3 O45 113.0(12) . . ?
O55 P3 C3 108.0(11) . . ?
O32 K1 Mn1 122.6(4) 2_556 7_567 ?
O43 K1 Mn1 98.4(4) 2_556 7_567 ?
O43 K1 O32 73.8(6) 2_556 2_556 ?
O43 K1 O46 140.9(7) 2_556 . ?
O43 K1 O52 65.0(6) 2_556 7_567 ?
O43 K1 O11W 65.4(10) 2_556 . ?
O46 K1 Mn1 84.7(4) . 7_567 ?
O46 K1 O32 136.2(6) . 2_556 ?
O46 K1 O52 116.4(7) . 7_567 ?
O52 K1 Mn1 34.7(4) 7_567 7_567 ?
O52 K1 O32 101.7(6) 7_567 2_556 ?
O53 K1 Mn1 34.9(4) 7_567 7_567 ?
O53 K1 O32 109.5(6) 7_567 2_556 ?
O53 K1 O43 128.6(6) 7_567 2_556 ?
O53 K1 O46 72.2(6) 7_567 . ?
O53 K1 O52 64.2(6) 7_567 7_567 ?
O53 K1 O9W 90.7(7) 7_567 1_556 ?
O53 K1 O11W 115.0(10) 7_567 . ?
O9W K1 Mn1 125.5(7) 1_556 7_567 ?
O9W K1 O32 67.0(7) 1_556 2_556 ?
O9W K1 O43 132.1(8) 1_556 2_556 ?
O9W K1 O46 69.2(7) 1_556 . ?
O9W K1 O52 148.3(7) 1_556 7_567 ?
O9W K1 O11W 127.2(10) 1_556 . ?
O11W K1 Mn1 87.9(8) . 7_567 ?
O11W K1 O32 132.2(10) . 2_556 ?
O11W K1 O46 75.9(10) . . ?
O11W K1 O52 83.0(9) . 7_567 ?
O22 K2 O25 113.6(8) 7_566 . ?
O22 K2 O6W 141.4(9) 7_566 . ?
O22 K2 O15W 74.8(12) 7_566 7_566 ?
O22 K2 O15W 110.4(11) 7_566 8_465 ?
O25 K2 O15W 136.0(12) . 8_465 ?
O25 K2 O15W 129.3(12) . 7_566 ?
O34 K2 O22 71.8(6) 7_566 7_566 ?
O34 K2 O25 68.2(6) 7_566 . ?
O34 K2 O39 104.4(8) 7_566 . ?
O34 K2 O6W 140.5(9) 7_566 . ?
O34 K2 O15W 68.1(12) 7_566 7_566 ?
O34 K2 O15W 127.1(11) 7_566 8_465 ?
O39 K2 O22 72.0(6) . 7_566 ?
O39 K2 O25 69.6(6) . . ?
O39 K2 O6W 77.7(8) . . ?
O39 K2 O15W 146.6(12) . 7_566 ?
O39 K2 O15W 127.1(11) . 8_465 ?
O6W K2 O25 76.2(9) . . ?
O6W K2 O15W 70.2(13) . 8_465 ?
O6W K2 O15W 129.6(15) . 7_566 ?
O15W K2 O15W 62.5(19) 7_566 8_465 ?
C1 N1 C3 108.0(19) . . ?
C2 N1 C1 112.4(18) . . ?
C2 N1 C3 110.3(18) . . ?
W2 O2 W1 121.3(8) . . ?
W3 O3 W1 121.0(9) . . ?
W1 O4 W13 145.1(9) . . ?
W9 O5 W1 151.9(9) . . ?
W1 O6 W3 90.4(5) . . ?
W2 O6 W1 91.4(5) . . ?
W2 O6 W3 90.6(5) . . ?
As1 O6 W1 118.3(8) . . ?
As1 O6 W2 120.1(8) . . ?
As1 O6 W3 135.0(8) . . ?
W3 O8 W2 120.5(8) . . ?
W4 O9 W2 151.1(11) . . ?
W2 O10 W14 147.5(9) . . ?
W8 O12 W3 148.1(11) . . ?
W3 O13 W5 155.3(11) . . ?
W5 O15 W4 122.9(10) . . ?
W6 O16 W4 120.8(9) . . ?
W4 O17 Mn1 156.8(12) . . ?
W4 O18 W5 92.9(6) . . ?
W4 O18 W6 92.9(7) . . ?
W6 O18 W5 90.4(5) . . ?
As1 O18 W4 119.1(7) . . ?
As1 O18 W5 133.4(9) . . ?
As1 O18 W6 118.2(7) . . ?
W6 O20 W5 122.1(9) . . ?
W8 O21 W5 149.5(10) . . ?
W6 O22 K2 142.8(9) . 7_566 ?
W7 O23 W6 158.8(9) . . ?
W6 O24 W10 148.7(12) . . ?
W7 O25 K2 136.8(10) . . ?
W7 O26 W8 121.3(9) . . ?
W7 O27 W9 121.4(9) . . ?
W11 O28 W7 151.0(10) . . ?
W7 O30 W8 91.0(4) . . ?
W7 O30 W9 91.9(6) . . ?
W9 O30 W8 90.8(6) . . ?
As1 O30 W7 119.8(8) . . ?
As1 O30 W8 134.0(8) . . ?
As1 O30 W9 118.7(7) . . ?
W9 O31 W8 123.8(10) . . ?
W9 O32 K1 141.4(9) . 2_556 ?
W12 O33 W9 154.5(10) . . ?
W10 O34 K2 139.2(9) . 7_566 ?
W11 O35 W10 148.0(10) . . ?
W10 O36 Mn1 111.8(9) . . ?
Mn1 O37 W10 90.4(6) . . ?
P1 O37 W10 138.3(9) . . ?
P1 O37 Mn1 128.4(8) . . ?
P2 O38 W10 135.2(9) . . ?
W11 O39 K2 138.8(9) . . ?
W12 O40 W11 122.1(10) . . ?
W12 O41 W11 92.8(6) . . ?
P1 O41 W11 131.5(10) . . ?
P1 O41 W12 134.4(9) . . ?
P3 O42 W11 136.2(11) . . ?
W12 O43 K1 147.7(11) . 2_556 ?
W12 O44 W13 153.1(10) . . ?
P3 O45 W12 134.0(11) . . ?
W13 O46 K1 145.5(9) . . ?
W13 O47 W14 123.3(8) . . ?
W14 O48 W13 91.0(5) . . ?
P1 O48 W13 131.9(10) . . ?
P1 O48 W14 135.4(10) . . ?
W13 O50 W14 159.8(13) 7_567 . ?
W14 O51 Mn1 147.7(10) . . ?
Mn1 O52 K1 91.0(7) . 7_567 ?
Mn1 O53 K1 99.1(6) . 7_567 ?
P2 O53 Mn1 127.9(9) . . ?
P2 O53 K1 128.8(10) . 7_567 ?
P1 C1 H1A 108.5 . . ?
P1 C1 H1B 108.5 . . ?
N1 C1 P1 115.2(15) . . ?
N1 C1 H1A 108.5 . . ?
N1 C1 H1B 108.5 . . ?
H1A C1 H1B 107.5 . . ?
N1 C2 P2 111.2(16) . . ?
P3 C3 H3A 109.5 . . ?
P3 C3 H3B 109.5 . . ?
N1 C3 P3 110.7(14) . . ?
N1 C3 H3A 109.5 . . ?
N1 C3 H3B 109.5 . . ?
H3A C3 H3B 108.1 . . ?
K2 O15W K2 112.3(18) 7_566 8_566 ?

_shelx_SHELXL_version_number     2014/7
_olex2_submission_special_instructions 'No special instructions were received'
